#------------------------------------------------------------------------------
#$Date: 2018-12-07 05:37:15 +0200 (Fri, 07 Dec 2018) $
#$Revision: 212436 $
#$URL: file:///home/coder/svn-repositories/cod/cif/2/10/83/2108346.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2108346
loop_
_publ_author_name
'Siidra, Oleg I.'
'Kozin, Michael S.'
'Depmeier, Wulf'
'Kayukov, Roman A.'
'Kovrugin, Vadim M.'
_publ_section_title
;
 Copper--lead selenite bromides: a new large family of compounds partly
 having Cu²⁺ substructures derivable from kagome nets
;
_journal_issue                   6
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              712
_journal_page_last               724
_journal_paper_doi               10.1107/S2052520618016542
_journal_volume                  74
_journal_year                    2018
_chemical_formula_sum            'Br1.17 Cu1.92 O3 Pb0.25 Se0.75'
_chemical_formula_weight         375.23
_space_group_crystal_system      monoclinic
_space_group_IT_number           12
_space_group_name_Hall           '-C 2y'
_space_group_name_H-M_alt        'C 1 2/m 1'
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_audit_creation_method           SHELXL-2014/7
_cell_angle_alpha                90
_cell_angle_beta                 99.270(7)
_cell_angle_gamma                90
_cell_formula_units_Z            16
_cell_length_a                   19.146(5)
_cell_length_b                   6.2686(18)
_cell_length_c                   17.296(5)
_cell_measurement_reflns_used    2300
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      27.999
_cell_measurement_theta_min      2.156
_cell_volume                     2048.7(10)
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 0.994
_diffrn_measured_fraction_theta_max 0.989
_diffrn_measurement_device_type  'Bruker Apex 2 Duo'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0461
_diffrn_reflns_av_unetI/netI     0.0510
_diffrn_reflns_Laue_measured_fraction_full 0.994
_diffrn_reflns_Laue_measured_fraction_max 0.989
_diffrn_reflns_limit_h_max       25
_diffrn_reflns_limit_h_min       -25
_diffrn_reflns_limit_k_max       8
_diffrn_reflns_limit_k_min       -5
_diffrn_reflns_limit_l_max       22
_diffrn_reflns_limit_l_min       -22
_diffrn_reflns_number            8910
_diffrn_reflns_point_group_measured_fraction_full 0.994
_diffrn_reflns_point_group_measured_fraction_max 0.989
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         27.999
_diffrn_reflns_theta_min         2.156
_exptl_absorpt_coefficient_mu    30.557
_exptl_crystal_density_diffrn    4.866
_exptl_crystal_description       prism
_exptl_crystal_F_000             2671
_refine_diff_density_max         3.111
_refine_diff_density_min         -1.747
_refine_diff_density_rms         0.429
_refine_ls_extinction_coef       0.000032(16)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2014/7 (Sheldrick 2014'
_refine_ls_goodness_of_fit_ref   1.060
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     174
_refine_ls_number_reflns         2683
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.060
_refine_ls_R_factor_all          0.0452
_refine_ls_R_factor_gt           0.0284
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0260P)²+0.7924P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0577
_refine_ls_wR_factor_ref         0.0632
_reflns_Friedel_coverage         0.000
_reflns_number_gt                2143
_reflns_number_total             2683
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            ps5074sup1.cif
_cod_data_source_block           CuPbOXO2
_cod_database_code               2108346
_shelx_shelxl_version_number     2014/7
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y, -z'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z'
'-x, -y, -z'
'x, -y, z'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
Pb1 Pb -0.00157(2) 0.0000 0.20810(2) 0.01048(10) Uani 1 2 d S T P
Se1 Se 0.03402(5) -0.5000 0.33955(5) 0.0081(2) Uani 1 2 d S T P
Se2 Se -0.22614(5) -0.5000 -0.29428(6) 0.0086(2) Uani 1 2 d S T P
Se3 Se -0.10201(5) 0.0000 -0.00694(6) 0.0089(2) Uani 1 2 d S T P
Br1 Br -0.19101(5) -0.5000 0.52006(6) 0.0169(2) Uani 1 2 d S T P
Br2 Br -0.35666(5) -0.5000 0.33619(6) 0.0156(2) Uani 1 2 d S T P
Br3 Br -0.05028(5) -0.5000 -0.13761(7) 0.0209(2) Uani 1 2 d S T P
Br4 Br -0.17479(6) -0.5000 0.16059(6) 0.0193(2) Uani 1 2 d S T P
Cu1 Cu -0.23210(6) -0.5000 0.34696(7) 0.0114(3) Uani 1 2 d S T P
Cu2 Cu -0.08036(6) -0.5000 0.46662(7) 0.0192(3) Uani 1 2 d S T P
Cu3 Cu -0.32076(6) -0.5000 -0.14988(7) 0.0113(3) Uani 1 2 d S T P
Cu4 Cu -0.11735(4) -0.24737(10) 0.30549(5) 0.01011(18) Uani 1 1 d . . .
Cu5 Cu -0.16051(6) -0.5000 -0.09476(7) 0.0151(3) Uani 1 2 d S T P
Cu6 Cu -0.2500 -0.2500 0.0000 0.0124(3) Uani 1 2 d S . P
Br5A Br -0.08625(12) 0.0000 0.45461(12) 0.0124(4) Uani 0.6 2 d S T P
Br5B Br -0.0651(7) 0.0000 0.4759(8) 0.011(3) Uiso 0.1 2 d S . P
Cu7 Cu -0.17933(16) -0.0851(4) 0.52093(17) 0.0333(7) Uani 0.35 1 d . . P
O1 O -0.1102(3) 0.0000 0.2433(4) 0.0074(13) Uani 1 2 d S T P
O2 O -0.2501(3) -0.5000 -0.0598(4) 0.0106(14) Uani 1 2 d S T P
O3 O -0.1291(3) -0.5000 0.3633(4) 0.0087(13) Uani 1 2 d S T P
O4 O -0.2322(3) -0.5000 -0.1981(4) 0.0134(14) Uani 1 2 d S T P
O5 O 0.0156(3) -0.5000 0.4342(4) 0.0135(14) Uani 1 2 d S T P
O6 O -0.0159(2) -0.2893(6) 0.3014(3) 0.0114(10) Uani 1 1 d . . .
O7 O -0.0970(3) 0.0000 0.0916(4) 0.0122(14) Uani 1 2 d S T P
O8 O -0.2827(2) -0.2978(6) -0.3270(3) 0.0130(10) Uani 1 1 d . . .
O9 O -0.1565(2) -0.2090(7) -0.0333(3) 0.0159(11) Uani 1 1 d . . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Se Se -0.0929 2.2259 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Br Br -0.2901 2.4595 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Pb Pb -3.3944 10.1111 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O1 Pb1 O6 67.70(14) . .
O1 Pb1 O6 67.70(14) . 6
O6 Pb1 O6 94.4(2) . 6
O1 Pb1 O7 68.3(2) . .
O6 Pb1 O7 112.56(13) . .
O6 Pb1 O7 112.56(13) 6 .
O1 Pb1 Br2 122.46(16) . 3
O6 Pb1 Br2 74.22(10) . 3
O6 Pb1 Br2 74.22(10) 6 3
O7 Pb1 Br2 169.22(15) . 3
O1 Pb1 Cu4 32.57(8) . .
O6 Pb1 Cu4 35.42(10) . .
O6 Pb1 Cu4 81.96(10) 6 .
O7 Pb1 Cu4 87.04(13) . .
Br2 Pb1 Cu4 102.51(3) 3 .
O1 Pb1 Cu4 32.57(8) . 6
O6 Pb1 Cu4 81.96(10) . 6
O6 Pb1 Cu4 35.42(10) 6 6
O7 Pb1 Cu4 87.04(13) . 6
Br2 Pb1 Cu4 102.51(3) 3 6
Cu4 Pb1 Cu4 54.79(3) . 6
O1 Pb1 Cu3 32.47(16) . 7_445
O6 Pb1 Cu3 88.99(10) . 7_445
O6 Pb1 Cu3 88.99(10) 6 7_445
O7 Pb1 Cu3 35.86(15) . 7_445
Br2 Pb1 Cu3 154.93(3) 3 7_445
Cu4 Pb1 Cu3 55.87(3) . 7_445
Cu4 Pb1 Cu3 55.87(3) 6 7_445
O1 Pb1 Br3 114.31(5) . 5_545
O6 Pb1 Br3 69.16(10) . 5_545
O6 Pb1 Br3 159.29(10) 6 5_545
O7 Pb1 Br3 86.09(7) . 5_545
Br2 Pb1 Br3 88.80(2) 3 5_545
Cu4 Pb1 Br3 90.47(3) . 5_545
Cu4 Pb1 Br3 144.89(2) 6 5_545
Cu3 Pb1 Br3 102.71(2) 7_445 5_545
O1 Pb1 Br3 114.31(5) . 5
O6 Pb1 Br3 159.30(10) . 5
O6 Pb1 Br3 69.16(10) 6 5
O7 Pb1 Br3 86.09(7) . 5
Br2 Pb1 Br3 88.80(2) 3 5
Cu4 Pb1 Br3 144.89(2) . 5
Cu4 Pb1 Br3 90.47(2) 6 5
Cu3 Pb1 Br3 102.71(2) 7_445 5
Br3 Pb1 Br3 123.28(4) 5_545 5
O6 Se1 O6 102.0(3) 6_545 .
O6 Se1 O5 100.4(2) 6_545 .
O6 Se1 O5 100.4(2) . .
O6 Se1 O3 63.43(16) 6_545 .
O6 Se1 O3 63.43(16) . .
O5 Se1 O3 61.9(2) . .
O6 Se1 Cu4 83.10(15) 6_545 .
O6 Se1 Cu4 29.28(15) . .
O5 Se1 Cu4 82.01(19) . .
O3 Se1 Cu4 34.15(6) . .
O6 Se1 Cu4 29.28(15) 6_545 6_545
O6 Se1 Cu4 83.10(15) . 6_545
O5 Se1 Cu4 82.01(19) . 6_545
O3 Se1 Cu4 34.15(6) . 6_545
Cu4 Se1 Cu4 57.90(3) . 6_545
O6 Se1 Cu2 115.66(16) 6_545 5_546
O6 Se1 Cu2 115.67(16) . 5_546
O5 Se1 Cu2 26.8(2) . 5_546
O3 Se1 Cu2 88.74(12) . 5_546
Cu4 Se1 Cu2 105.44(3) . 5_546
Cu4 Se1 Cu2 105.44(3) 6_545 5_546
O6 Se1 Cu2 82.43(16) 6_545 .
O6 Se1 Cu2 82.44(16) . .
O5 Se1 Cu2 28.7(2) . .
O3 Se1 Cu2 33.20(11) . .
Cu4 Se1 Cu2 57.54(3) . .
Cu4 Se1 Cu2 57.54(3) 6_545 .
Cu2 Se1 Cu2 55.54(4) 5_546 .
O6 Se1 Br1 128.84(15) 6_545 5_546
O6 Se1 Br1 128.84(15) . 5_546
O5 Se1 Br1 68.3(2) . 5_546
O3 Se1 Br1 130.24(12) . 5_546
Cu4 Se1 Br1 138.74(3) . 5_546
Cu4 Se1 Br1 138.74(3) 6_545 5_546
Cu2 Se1 Br1 41.50(3) 5_546 5_546
Cu2 Se1 Br1 97.04(4) . 5_546
O6 Se1 Br3 75.61(16) 6_545 5_545
O6 Se1 Br3 75.61(16) . 5_545
O5 Se1 Br3 173.4(2) . 5_545
O3 Se1 Br3 111.47(11) . 5_545
Cu4 Se1 Br3 92.19(3) . 5_545
Cu4 Se1 Br3 92.19(3) 6_545 5_545
Cu2 Se1 Br3 159.79(4) 5_546 5_545
Cu2 Se1 Br3 144.68(4) . 5_545
Br1 Se1 Br3 118.28(4) 5_546 5_545
O4 Se2 O8 100.8(2) . .
O4 Se2 O8 100.8(2) . 6_545
O8 Se2 O8 96.2(3) . 6_545
O4 Se2 Cu3 28.8(2) . .
O8 Se2 Cu3 81.64(16) . .
O8 Se2 Cu3 81.64(16) 6_545 .
O4 Se2 Cu1 102.63(6) . 7_435
O8 Se2 Cu1 119.90(15) . 7_435
O8 Se2 Cu1 25.28(14) 6_545 7_435
Cu3 Se2 Cu1 94.01(3) . 7_435
O4 Se2 Cu1 102.63(6) . 7_445
O8 Se2 Cu1 25.28(14) . 7_445
O8 Se2 Cu1 119.90(15) 6_545 7_445
Cu3 Se2 Cu1 94.01(3) . 7_445
Cu1 Se2 Cu1 140.96(5) 7_435 7_445
O4 Se2 Cu4 81.6(2) . 4_445
O8 Se2 Cu4 79.08(15) . 4_445
O8 Se2 Cu4 28.59(15) 6_545 4_445
Cu3 Se2 Cu4 56.72(3) . 4_445
Cu1 Se2 Cu4 51.31(2) 7_435 4_445
Cu1 Se2 Cu4 104.30(4) 7_445 4_445
O4 Se2 Cu4 81.6(2) . 7_445
O8 Se2 Cu4 28.59(15) . 7_445
O8 Se2 Cu4 79.07(15) 6_545 7_445
Cu3 Se2 Cu4 56.72(3) . 7_445
Cu1 Se2 Cu4 104.30(4) 7_435 7_445
Cu1 Se2 Cu4 51.31(2) 7_445 7_445
Cu4 Se2 Cu4 55.12(3) 4_445 7_445
O4 Se2 Br1 172.6(2) . 1_554
O8 Se2 Br1 84.14(16) . 1_554
O8 Se2 Br1 84.14(16) 6_545 1_554
Cu3 Se2 Br1 158.65(4) . 1_554
Cu1 Se2 Br1 79.39(3) 7_435 1_554
Cu1 Se2 Br1 79.39(3) 7_445 1_554
Cu4 Se2 Br1 104.92(3) 4_445 1_554
Cu4 Se2 Br1 104.92(3) 7_445 1_554
O4 Se2 O1 62.0(2) . 7_445
O8 Se2 O1 61.41(16) . 7_445
O8 Se2 O1 61.41(16) 6_545 7_445
Cu3 Se2 O1 33.18(11) . 7_445
Cu1 Se2 O1 83.09(4) 7_435 7_445
Cu1 Se2 O1 83.09(4) 7_445 7_445
Cu4 Se2 O1 32.82(6) 4_445 7_445
Cu4 Se2 O1 32.82(6) 7_445 7_445
Br1 Se2 O1 125.46(11) 1_554 7_445
O4 Se2 Cu5 24.8(2) . .
O8 Se2 Cu5 115.98(16) . .
O8 Se2 Cu5 115.98(16) 6_545 .
Cu3 Se2 Cu5 53.55(4) . .
Cu1 Se2 Cu5 107.72(3) 7_435 .
Cu1 Se2 Cu5 107.72(3) 7_445 .
Cu4 Se2 Cu5 103.54(3) 4_445 .
Cu4 Se2 Cu5 103.54(3) 7_445 .
Br1 Se2 Cu5 147.80(4) 1_554 .
O1 Se2 Cu5 86.73(11) 7_445 .
O4 Se2 Br2 107.33(10) . 7_445
O8 Se2 Br2 64.33(14) . 7_445
O8 Se2 Br2 148.12(16) 6_545 7_445
Cu3 Se2 Br2 117.32(2) . 7_445
Cu1 Se2 Br2 148.30(4) 7_435 7_445
Cu1 Se2 Br2 39.34(3) 7_445 7_445
Cu4 Se2 Br2 143.26(3) 4_445 7_445
Cu4 Se2 Br2 90.23(3) 7_445 7_445
Br1 Se2 Br2 69.60(2) 1_554 7_445
O1 Se2 Br2 120.18(2) 7_445 7_445
Cu5 Se2 Br2 95.65(3) . 7_445
O9 Se3 O9 101.6(3) . 6
O9 Se3 O7 101.8(2) . .
O9 Se3 O7 101.8(2) 6 .
O9 Se3 O2 63.74(17) . 7_445
O9 Se3 O2 63.74(17) 6 7_445
O7 Se3 O2 63.2(2) . 7_445
O9 Se3 Cu6 30.07(16) . .
O9 Se3 Cu6 83.11(16) 6 .
O7 Se3 Cu6 82.59(18) . .
O2 Se3 Cu6 33.67(6) 7_445 .
O9 Se3 Cu6 83.11(16) . 4_455
O9 Se3 Cu6 30.07(16) 6 4_455
O7 Se3 Cu6 82.59(18) . 4_455
O2 Se3 Cu6 33.67(6) 7_445 4_455
Cu6 Se3 Cu6 57.52(2) . 4_455
O9 Se3 Cu3 83.27(17) . 7_445
O9 Se3 Cu3 83.27(17) 6 7_445
O7 Se3 Cu3 29.5(2) . 7_445
O2 Se3 Cu3 33.72(12) 7_445 7_445
Cu6 Se3 Cu3 57.37(2) . 7_445
Cu6 Se3 Cu3 57.37(2) 4_455 7_445
O9 Se3 Cu5 115.23(16) . 1_565
O9 Se3 Cu5 21.69(16) 6 1_565
O7 Se3 Cu5 112.96(7) . 1_565
O2 Se3 Cu5 85.37(6) 7_445 1_565
Cu6 Se3 Cu5 102.84(3) . 1_565
Cu6 Se3 Cu5 51.71(2) 4_455 1_565
Cu3 Se3 Cu5 101.43(3) 7_445 1_565
O9 Se3 Cu5 21.69(16) . .
O9 Se3 Cu5 115.23(16) 6 .
O7 Se3 Cu5 112.96(7) . .
O2 Se3 Cu5 85.37(6) 7_445 .
Cu6 Se3 Cu5 51.71(2) . .
Cu6 Se3 Cu5 102.84(3) 4_455 .
Cu3 Se3 Cu5 101.43(3) 7_445 .
Cu5 Se3 Cu5 122.04(5) 1_565 .
Cu2 Br1 Cu7 140.02(8) . 4_446
Cu2 Br1 Cu7 140.02(8) . 7_446
Cu7 Br1 Cu7 24.38(12) 4_446 7_446
Cu2 Br1 Cu7 85.61(7) . 6_545
Cu7 Br1 Cu7 82.57(10) 4_446 6_545
Cu7 Br1 Cu7 106.94(9) 7_446 6_545
Cu2 Br1 Cu7 85.61(7) . .
Cu7 Br1 Cu7 106.94(9) 4_446 .
Cu7 Br1 Cu7 82.57(10) 7_446 .
Cu7 Br1 Cu7 170.25(14) 6_545 .
Cu2 Br1 Cu1 73.96(5) . .
Cu7 Br1 Cu1 68.19(7) 4_446 .
Cu7 Br1 Cu1 68.19(7) 7_446 .
Cu7 Br1 Cu1 90.82(7) 6_545 .
Cu7 Br1 Cu1 90.82(7) . .
Cu2 Br1 O3 36.86(12) . .
Cu7 Br1 O3 104.42(13) 4_446 .
Cu7 Br1 O3 104.42(13) 7_446 .
Cu7 Br1 O3 87.76(7) 6_545 .
Cu7 Br1 O3 87.76(7) . .
Cu1 Br1 O3 37.11(12) . .
Cu2 Br1 O5 35.50(12) . 5_546
Cu7 Br1 O5 167.48(7) 4_446 5_546
Cu7 Br1 O5 167.48(7) 7_446 5_546
Cu7 Br1 O5 85.20(7) 6_545 5_546
Cu7 Br1 O5 85.20(7) . 5_546
Cu1 Br1 O5 109.46(12) . 5_546
O3 Br1 O5 72.35(16) . 5_546
Cu2 Br1 Se2 132.49(5) . 1_556
Cu7 Br1 Se2 85.98(7) 4_446 1_556
Cu7 Br1 Se2 85.98(7) 7_446 1_556
Cu7 Br1 Se2 91.40(7) 6_545 1_556
Cu7 Br1 Se2 91.40(7) . 1_556
Cu1 Br1 Se2 153.54(5) . 1_556
O3 Br1 Se2 169.35(12) . 1_556
O5 Br1 Se2 97.00(12) 5_546 1_556
Cu2 Br1 Se1 64.42(4) . 5_546
Cu7 Br1 Se1 151.43(7) 4_446 5_546
Cu7 Br1 Se1 151.43(7) 7_446 5_546
Cu7 Br1 Se1 86.20(7) 6_545 5_546
Cu7 Br1 Se1 86.20(7) . 5_546
Cu1 Br1 Se1 138.39(4) . 5_546
O3 Br1 Se1 101.28(12) . 5_546
O5 Br1 Se1 28.93(11) 5_546 5_546
Se2 Br1 Se1 68.07(3) 1_556 5_546
Cu2 Br1 O8 145.67(8) . 1_556
Cu7 Br1 O8 73.12(10) 4_446 1_556
Cu7 Br1 O8 64.04(10) 7_446 1_556
Cu7 Br1 O8 113.25(9) 6_545 1_556
Cu7 Br1 O8 72.48(9) . 1_556
Cu1 Br1 O8 130.83(8) . 1_556
O3 Br1 O8 157.88(8) . 1_556
O5 Br1 O8 114.53(13) 5_546 1_556
Se2 Br1 O8 27.82(7) 1_556 1_556
Se1 Br1 O8 87.54(8) 5_546 1_556
Cu2 Br1 O8 145.67(8) . 6_546
Cu7 Br1 O8 64.04(10) 4_446 6_546
Cu7 Br1 O8 73.12(10) 7_446 6_546
Cu7 Br1 O8 72.48(9) 6_545 6_546
Cu7 Br1 O8 113.25(9) . 6_546
Cu1 Br1 O8 130.83(8) . 6_546
O3 Br1 O8 157.88(8) . 6_546
O5 Br1 O8 114.53(13) 5_546 6_546
Se2 Br1 O8 27.82(7) 1_556 6_546
Se1 Br1 O8 87.54(8) 5_546 6_546
O8 Br1 O8 40.87(12) 1_556 6_546
Cu1 Br2 Cu7 79.00(8) . 7_446
Cu1 Br2 Cu7 79.00(8) . 4_446
Cu7 Br2 Cu7 24.51(13) 7_446 4_446
Cu1 Br2 Pb1 142.33(5) . 3_445
Cu7 Br2 Pb1 137.46(8) 7_446 3_445
Cu7 Br2 Pb1 137.46(8) 4_446 3_445
Cu1 Br2 O8 35.43(7) . 7_445
Cu7 Br2 O8 80.26(11) 7_446 7_445
Cu7 Br2 O8 94.14(11) 4_446 7_445
Pb1 Br2 O8 125.22(9) 3_445 7_445
Cu1 Br2 O8 35.43(7) . 4_445
Cu7 Br2 O8 94.14(11) 7_446 4_445
Cu7 Br2 O8 80.26(11) 4_446 4_445
Pb1 Br2 O8 125.22(9) 3_445 4_445
O8 Br2 O8 69.34(14) 7_445 4_445
Cu1 Br2 O6 148.25(7) . 3_445
Cu7 Br2 O6 111.76(10) 7_446 3_445
Cu7 Br2 O6 98.72(10) 4_446 3_445
Pb1 Br2 O6 42.60(7) 3_445 3_445
O8 Br2 O6 167.14(11) 7_445 3_445
O8 Br2 O6 112.82(10) 4_445 3_445
Cu1 Br2 O6 148.25(7) . 8_445
Cu7 Br2 O6 98.72(10) 7_446 8_445
Cu7 Br2 O6 111.76(10) 4_446 8_445
Pb1 Br2 O6 42.60(7) 3_445 8_445
O8 Br2 O6 112.82(10) 7_445 8_445
O8 Br2 O6 167.14(11) 4_445 8_445
O6 Br2 O6 62.13(13) 3_445 8_445
Cu1 Br2 Se2 63.18(2) . 7_445
Cu7 Br2 Se2 87.35(7) 7_446 7_445
Cu7 Br2 Se2 108.64(7) 4_446 7_445
Pb1 Br2 Se2 102.42(3) 3_445 7_445
O8 Br2 Se2 27.91(7) 7_445 7_445
O8 Br2 Se2 95.54(8) 4_445 7_445
O6 Br2 Se2 143.54(7) 3_445 7_445
O6 Br2 Se2 85.13(7) 8_445 7_445
Cu1 Br2 Se2 63.18(2) . 7_435
Cu7 Br2 Se2 108.64(7) 7_446 7_435
Cu7 Br2 Se2 87.35(7) 4_446 7_435
Pb1 Br2 Se2 102.42(3) 3_445 7_435
O8 Br2 Se2 95.54(8) 7_445 7_435
O8 Br2 Se2 27.91(7) 4_445 7_435
O6 Br2 Se2 85.13(7) 3_445 7_435
O6 Br2 Se2 143.54(7) 8_445 7_435
Se2 Br2 Se2 119.00(4) 7_445 7_435
Cu1 Br2 Br5B 117.8(2) . 7_446
Cu7 Br2 Br5B 40.60(19) 7_446 7_446
Cu7 Br2 Br5B 40.60(19) 4_446 7_446
Pb1 Br2 Br5B 99.92(19) 3_445 7_446
O8 Br2 Br5B 118.57(17) 7_445 7_446
O8 Br2 Br5B 118.57(17) 4_445 7_446
O6 Br2 Br5B 72.26(18) 3_445 7_446
O6 Br2 Br5B 72.26(18) 8_445 7_446
Se2 Br2 Br5B 114.57(7) 7_445 7_446
Se2 Br2 Br5B 114.57(7) 7_435 7_446
Cu1 Br2 Br5A 110.68(6) . 7_446
Cu7 Br2 Br5A 33.98(8) 7_446 7_446
Cu7 Br2 Br5A 33.98(8) 4_446 7_446
Pb1 Br2 Br5A 106.99(5) 3_445 7_446
O8 Br2 Br5A 113.09(9) 7_445 7_446
O8 Br2 Br5A 113.09(9) 4_445 7_446
O6 Br2 Br5A 78.24(8) 3_445 7_446
O6 Br2 Br5A 78.24(8) 8_445 7_446
Se2 Br2 Br5A 112.14(3) 7_445 7_446
Se2 Br2 Br5A 112.14(3) 7_435 7_446
Br5B Br2 Br5A 7.07(19) 7_446 7_446
Cu5 Br3 O9 36.77(7) . .
Cu5 Br3 O9 36.76(7) . 6_545
O9 Br3 O9 63.85(15) . 6_545
Cu5 Br3 O4 35.46(11) . .
O9 Br3 O4 60.67(12) . .
O9 Br3 O4 60.67(12) 6_545 .
Cu5 Br3 O6 135.13(8) . 5_545
O9 Br3 O6 158.89(11) . 5_545
O9 Br3 O6 122.57(10) 6_545 5_545
O4 Br3 O6 103.29(13) . 5_545
Cu5 Br3 O6 135.13(8) . 2
O9 Br3 O6 122.57(10) . 2
O9 Br3 O6 158.89(11) 6_545 2
O4 Br3 O6 103.29(13) . 2
O6 Br3 O6 43.81(13) 5_545 2
Cu5 Br3 Se1 122.39(5) . 5_545
O9 Br3 Se1 131.75(8) . 5_545
O9 Br3 Se1 131.75(8) 6_545 5_545
O4 Br3 Se1 86.93(11) . 5_545
O6 Br3 Se1 27.72(7) 5_545 5_545
O6 Br3 Se1 27.72(7) 2 5_545
Cu5 Br3 Pb1 115.00(2) . 5_545
O9 Br3 Pb1 149.85(7) . 5_545
O9 Br3 Pb1 86.22(7) 6_545 5_545
O4 Br3 Pb1 102.61(5) . 5_545
O6 Br3 Pb1 40.74(7) 5_545 5_545
O6 Br3 Pb1 84.20(7) 2 5_545
Se1 Br3 Pb1 65.824(19) 5_545 5_545
Cu5 Br3 Pb1 115.00(2) . 5
O9 Br3 Pb1 86.22(7) . 5
O9 Br3 Pb1 149.84(7) 6_545 5
O4 Br3 Pb1 102.61(5) . 5
O6 Br3 Pb1 84.20(7) 5_545 5
O6 Br3 Pb1 40.74(7) 2 5
Se1 Br3 Pb1 65.824(19) 5_545 5
Pb1 Br3 Pb1 123.28(4) 5_545 5
Cu5 Br3 O7 123.37(8) . 5
O9 Br3 O7 86.61(11) . 5
O9 Br3 O7 136.81(12) 6_545 5
O4 Br3 O7 131.81(6) . 5
O6 Br3 O7 96.54(11) 5_545 5
O6 Br3 O7 63.76(11) 2 5
Se1 Br3 O7 91.35(9) 5_545 5
Pb1 Br3 O7 120.34(8) 5_545 5
Pb1 Br3 O7 36.25(8) 5 5
Cu5 Br3 O7 123.37(8) . 5_545
O9 Br3 O7 136.81(12) . 5_545
O9 Br3 O7 86.61(11) 6_545 5_545
O4 Br3 O7 131.81(6) . 5_545
O6 Br3 O7 63.76(11) 5_545 5_545
O6 Br3 O7 96.54(11) 2 5_545
Se1 Br3 O7 91.35(9) 5_545 5_545
Pb1 Br3 O7 36.25(8) 5_545 5_545
Pb1 Br3 O7 120.34(8) 5 5_545
O7 Br3 O7 96.36(13) 5 5_545
Cu5 Br3 O2 0.02(9) . .
O9 Br3 O2 36.76(8) . .
O9 Br3 O2 36.76(8) 6_545 .
O4 Br3 O2 35.48(14) . .
O6 Br3 O2 135.15(11) 5_545 .
O6 Br3 O2 135.15(11) 2 .
Se1 Br3 O2 122.41(9) 5_545 .
Pb1 Br3 O2 115.00(3) 5_545 .
Pb1 Br3 O2 115.00(3) 5 .
O7 Br3 O2 123.36(9) 5 .
O7 Br3 O2 123.36(9) 5_545 .
Cu4 Br4 Cu4 63.29(4) . 6_545
Cu4 Br4 Cu3 125.13(4) . 7_435
Cu4 Br4 Cu3 61.84(3) 6_545 7_435
Cu4 Br4 Cu3 61.84(3) . 7_445
Cu4 Br4 Cu3 125.13(4) 6_545 7_445
Cu3 Br4 Cu3 173.02(6) 7_435 7_445
Cu4 Br4 Cu6 175.04(3) . 4_445
Cu4 Br4 Cu6 119.96(2) 6_545 4_445
Cu3 Br4 Cu6 58.26(3) 7_435 4_445
Cu3 Br4 Cu6 114.77(4) 7_445 4_445
Cu4 Br4 Cu6 119.96(2) . .
Cu4 Br4 Cu6 175.04(3) 6_545 .
Cu3 Br4 Cu6 114.77(4) 7_435 .
Cu3 Br4 Cu6 58.26(3) 7_445 .
Cu6 Br4 Cu6 56.52(3) 4_445 .
Cu4 Br4 O3 33.20(4) . .
Cu4 Br4 O3 33.20(4) 6_545 .
Cu3 Br4 O3 93.42(3) 7_435 .
Cu3 Br4 O3 93.42(3) 7_445 .
Cu6 Br4 O3 148.39(5) 4_445 .
Cu6 Br4 O3 148.39(5) . .
Cu4 Br4 Cu1 51.24(3) . .
Cu4 Br4 Cu1 51.24(3) 6_545 .
Cu3 Br4 Cu1 92.52(3) 7_435 .
Cu3 Br4 Cu1 92.52(3) 7_445 .
Cu6 Br4 Cu1 127.05(3) 4_445 .
Cu6 Br4 Cu1 127.05(3) . .
O3 Br4 Cu1 32.05(10) . .
Cu4 Br4 O1 32.13(9) . .
Cu4 Br4 O1 94.10(9) 6_545 .
Cu3 Br4 O1 154.34(10) 7_435 .
Cu3 Br4 O1 32.27(9) 7_445 .
Cu6 Br4 O1 145.58(9) 4_445 .
Cu6 Br4 O1 89.79(9) . .
O3 Br4 O1 65.32(10) . .
Cu1 Br4 O1 77.05(10) . .
Cu4 Br4 O1 94.10(9) . 1_545
Cu4 Br4 O1 32.13(9) 6_545 1_545
Cu3 Br4 O1 32.27(9) 7_435 1_545
Cu3 Br4 O1 154.34(10) 7_445 1_545
Cu6 Br4 O1 89.79(9) 4_445 1_545
Cu6 Br4 O1 145.58(9) . 1_545
O3 Br4 O1 65.32(10) . 1_545
Cu1 Br4 O1 77.05(10) . 1_545
O1 Br4 O1 122.12(18) . 1_545
Cu4 Br4 O8 33.94(7) . 7_445
Cu4 Br4 O8 73.13(7) 6_545 7_445
Cu3 Br4 O8 123.54(7) 7_435 7_445
Cu3 Br4 O8 61.72(7) 7_445 7_445
Cu6 Br4 O8 141.79(8) 4_445 7_445
Cu6 Br4 O8 107.40(7) . 7_445
O3 Br4 O8 41.60(9) . 7_445
Cu1 Br4 O8 31.04(6) . 7_445
O1 Br4 O8 48.75(12) . 7_445
O1 Br4 O8 103.91(12) 1_545 7_445
Cu4 Br4 O8 73.13(7) . 4_445
Cu4 Br4 O8 33.94(7) 6_545 4_445
Cu3 Br4 O8 61.72(7) 7_435 4_445
Cu3 Br4 O8 123.54(7) 7_445 4_445
Cu6 Br4 O8 107.40(7) 4_445 4_445
Cu6 Br4 O8 141.79(8) . 4_445
O3 Br4 O8 41.60(9) . 4_445
Cu1 Br4 O8 31.04(6) . 4_445
O1 Br4 O8 103.91(12) . 4_445
O1 Br4 O8 48.75(12) 1_545 4_445
O8 Br4 O8 61.87(13) 7_445 4_445
O8 Cu1 O8 151.1(3) 4_445 7_445
O8 Cu1 O3 81.44(14) 4_445 .
O8 Cu1 O3 81.44(14) 7_445 .
O8 Cu1 Br2 99.30(14) 4_445 .
O8 Cu1 Br2 99.30(14) 7_445 .
O3 Cu1 Br2 176.2(2) . .
O8 Cu1 Cu4 44.39(13) 4_445 6_545
O8 Cu1 Cu4 110.26(14) 7_445 6_545
O3 Cu1 Cu4 40.84(10) . 6_545
Br2 Cu1 Cu4 141.12(4) . 6_545
O8 Cu1 Cu4 110.26(14) 4_445 .
O8 Cu1 Cu4 44.39(13) 7_445 .
O3 Cu1 Cu4 40.84(10) . .
Br2 Cu1 Cu4 141.12(4) . .
Cu4 Cu1 Cu4 66.43(4) 6_545 .
O8 Cu1 Br1 99.09(15) 4_445 .
O8 Cu1 Br1 99.09(15) 7_445 .
O3 Cu1 Br1 75.87(19) . .
Br2 Cu1 Br1 100.34(5) . .
Cu4 Cu1 Br1 99.30(4) 6_545 .
Cu4 Cu1 Br1 99.30(4) . .
O8 Cu1 Cu7 114.34(15) 4_445 7_446
O8 Cu1 Cu7 94.54(15) 7_445 7_446
O3 Cu1 Cu7 123.6(2) . 7_446
Br2 Cu1 Cu7 52.66(7) . 7_446
Cu4 Cu1 Cu7 143.53(7) 6_545 7_446
Cu4 Cu1 Cu7 128.01(6) . 7_446
Br1 Cu1 Cu7 49.10(6) . 7_446
O8 Cu1 Cu7 94.54(15) 4_445 4_446
O8 Cu1 Cu7 114.34(15) 7_445 4_446
O3 Cu1 Cu7 123.6(2) . 4_446
Br2 Cu1 Cu7 52.66(7) . 4_446
Cu4 Cu1 Cu7 128.01(6) 6_545 4_446
Cu4 Cu1 Cu7 143.53(7) . 4_446
Br1 Cu1 Cu7 49.10(6) . 4_446
Cu7 Cu1 Cu7 19.80(10) 7_446 4_446
O8 Cu1 Cu2 88.41(14) 4_445 .
O8 Cu1 Cu2 88.41(14) 7_445 .
O3 Cu1 Cu2 30.21(19) . .
Br2 Cu1 Cu2 146.00(6) . .
Cu4 Cu1 Cu2 61.70(3) 6_545 .
Cu4 Cu1 Cu2 61.70(3) . .
Br1 Cu1 Cu2 45.66(3) . .
Cu7 Cu1 Cu2 93.94(7) 7_446 .
Cu7 Cu1 Cu2 93.94(7) 4_446 .
O8 Cu1 Se2 22.18(13) 4_445 7_435
O8 Cu1 Se2 154.08(16) 7_445 7_435
O3 Cu1 Se2 103.48(5) . 7_435
Br2 Cu1 Se2 77.48(3) . 7_435
Cu4 Cu1 Se2 64.82(3) 6_545 7_435
Cu4 Cu1 Se2 127.38(4) . 7_435
Br1 Cu1 Se2 106.80(3) . 7_435
Cu7 Cu1 Se2 103.18(6) 7_446 7_435
Cu7 Cu1 Se2 84.49(6) 4_446 7_435
Cu2 Cu1 Se2 108.78(3) . 7_435
O8 Cu1 Se2 154.08(16) 4_445 7_445
O8 Cu1 Se2 22.18(13) 7_445 7_445
O3 Cu1 Se2 103.48(5) . 7_445
Br2 Cu1 Se2 77.48(3) . 7_445
Cu4 Cu1 Se2 127.38(4) 6_545 7_445
Cu4 Cu1 Se2 64.82(3) . 7_445
Br1 Cu1 Se2 106.80(3) . 7_445
Cu7 Cu1 Se2 84.49(6) 7_446 7_445
Cu7 Cu1 Se2 103.18(6) 4_446 7_445
Cu2 Cu1 Se2 108.78(3) . 7_445
Se2 Cu1 Se2 140.96(5) 7_435 7_445
O3 Cu2 O5 170.5(3) . 5_546
O3 Cu2 O5 94.1(3) . .
O5 Cu2 O5 76.4(3) 5_546 .
O3 Cu2 Br1 91.8(2) . .
O5 Cu2 Br1 97.7(2) 5_546 .
O5 Cu2 Br1 174.09(19) . .
O3 Cu2 Cu2 131.6(2) . 5_546
O5 Cu2 Cu2 38.85(19) 5_546 5_546
O5 Cu2 Cu2 37.52(19) . 5_546
Br1 Cu2 Cu2 136.57(7) . 5_546
O3 Cu2 Br5A 85.99(5) . .
O5 Cu2 Br5A 93.97(5) 5_546 .
O5 Cu2 Br5A 90.36(5) . .
Br1 Cu2 Br5A 90.05(5) . .
Cu2 Cu2 Br5A 92.72(5) 5_546 .
O3 Cu2 Br5A 85.99(5) . 1_545
O5 Cu2 Br5A 93.97(5) 5_546 1_545
O5 Cu2 Br5A 90.36(5) . 1_545
Br1 Cu2 Br5A 90.05(5) . 1_545
Cu2 Cu2 Br5A 92.72(5) 5_546 1_545
Br5A Cu2 Br5A 171.98(9) . 1_545
O3 Cu2 Br5B 94.4(2) . .
O5 Cu2 Br5B 85.1(2) 5_546 .
O5 Cu2 Br5B 86.1(3) . .
Br1 Cu2 Br5B 93.4(3) . .
Cu2 Cu2 Br5B 84.4(2) 5_546 .
Br5A Cu2 Br5B 9.1(2) . .
Br5A Cu2 Br5B 176.5(2) 1_545 .
O3 Cu2 Br5B 94.4(2) . 1_545
O5 Cu2 Br5B 85.1(2) 5_546 1_545
O5 Cu2 Br5B 86.1(3) . 1_545
Br1 Cu2 Br5B 93.4(3) . 1_545
Cu2 Cu2 Br5B 84.4(2) 5_546 1_545
Br5A Cu2 Br5B 176.5(2) . 1_545
Br5A Cu2 Br5B 9.1(2) 1_545 1_545
Br5B Cu2 Br5B 168.7(5) . 1_545
O3 Cu2 Cu4 32.95(8) . 6_545
O5 Cu2 Cu4 142.28(12) 5_546 6_545
O5 Cu2 Cu4 80.80(16) . 6_545
Br1 Cu2 Cu4 104.29(4) . 6_545
Cu2 Cu2 Cu4 113.11(5) 5_546 6_545
Br5A Cu2 Cu4 115.96(5) . 6_545
Br5A Cu2 Cu4 56.33(4) 1_545 6_545
Br5B Cu2 Cu4 123.0(3) . 6_545
Br5B Cu2 Cu4 63.6(2) 1_545 6_545
O3 Cu2 Cu4 32.95(8) . .
O5 Cu2 Cu4 142.28(12) 5_546 .
O5 Cu2 Cu4 80.80(16) . .
Br1 Cu2 Cu4 104.29(4) . .
Cu2 Cu2 Cu4 113.11(5) 5_546 .
Br5A Cu2 Cu4 56.33(4) . .
Br5A Cu2 Cu4 115.96(5) 1_545 .
Br5B Cu2 Cu4 63.6(2) . .
Br5B Cu2 Cu4 123.0(3) 1_545 .
Cu4 Cu2 Cu4 59.64(4) 6_545 .
O3 Cu2 Cu1 31.44(19) . .
O5 Cu2 Cu1 158.1(2) 5_546 .
O5 Cu2 Cu1 125.54(19) . .
Br1 Cu2 Cu1 60.38(4) . .
Cu2 Cu2 Cu1 163.06(7) 5_546 .
Br5A Cu2 Cu1 86.54(5) . .
Br5A Cu2 Cu1 86.54(5) 1_545 .
Br5B Cu2 Cu1 95.6(2) . .
Br5B Cu2 Cu1 95.6(2) 1_545 .
Cu4 Cu2 Cu1 53.06(3) 6_545 .
Cu4 Cu2 Cu1 53.06(3) . .
O2 Cu3 O1 178.0(3) . 7_445
O2 Cu3 O7 95.8(3) . 7_445
O1 Cu3 O7 86.1(3) 7_445 7_445
O2 Cu3 O4 78.6(3) . .
O1 Cu3 O4 99.5(3) 7_445 .
O7 Cu3 O4 174.4(3) 7_445 .
O2 Cu3 Cu5 36.46(19) . .
O1 Cu3 Cu5 141.55(19) 7_445 .
O7 Cu3 Cu5 132.30(19) 7_445 .
O4 Cu3 Cu5 42.09(19) . .
O2 Cu3 Br4 93.30(3) . 7_435
O1 Cu3 Br4 86.66(3) 7_445 7_435
O7 Cu3 Br4 90.78(3) 7_445 7_435
O4 Cu3 Br4 89.55(3) . 7_435
Cu5 Cu3 Br4 91.99(3) . 7_435
O2 Cu3 Br4 93.30(3) . 7_445
O1 Cu3 Br4 86.66(3) 7_445 7_445
O7 Cu3 Br4 90.78(3) 7_445 7_445
O4 Cu3 Br4 89.55(3) . 7_445
Cu5 Cu3 Br4 91.99(3) . 7_445
Br4 Cu3 Br4 173.02(6) 7_435 7_445
O2 Cu3 Cu6 33.36(8) . .
O1 Cu3 Cu6 147.43(7) 7_445 .
O7 Cu3 Cu6 81.61(16) 7_445 .
O4 Cu3 Cu6 93.54(17) . .
Cu5 Cu3 Cu6 57.74(3) . .
Br4 Cu3 Cu6 123.39(4) 7_435 .
Br4 Cu3 Cu6 63.58(2) 7_445 .
O2 Cu3 Cu6 33.36(8) . 4_445
O1 Cu3 Cu6 147.43(7) 7_445 4_445
O7 Cu3 Cu6 81.61(16) 7_445 4_445
O4 Cu3 Cu6 93.54(17) . 4_445
Cu5 Cu3 Cu6 57.74(3) . 4_445
Br4 Cu3 Cu6 63.58(2) 7_435 4_445
Br4 Cu3 Cu6 123.39(4) 7_445 4_445
Cu6 Cu3 Cu6 59.81(3) . 4_445
O2 Cu3 Cu4 145.09(10) . 4_445
O1 Cu3 Cu4 33.92(9) 7_445 4_445
O7 Cu3 Cu4 102.19(17) 7_445 4_445
O4 Cu3 Cu4 82.68(17) . 4_445
Cu5 Cu3 Cu4 118.92(4) . 4_445
Br4 Cu3 Cu4 57.19(3) 7_435 4_445
Br4 Cu3 Cu4 115.84(4) 7_445 4_445
Cu6 Cu3 Cu4 176.20(4) . 4_445
Cu6 Cu3 Cu4 120.63(2) 4_445 4_445
O2 Cu3 Cu4 145.09(10) . 7_445
O1 Cu3 Cu4 33.92(9) 7_445 7_445
O7 Cu3 Cu4 102.19(17) 7_445 7_445
O4 Cu3 Cu4 82.68(17) . 7_445
Cu5 Cu3 Cu4 118.92(4) . 7_445
Br4 Cu3 Cu4 115.84(4) 7_435 7_445
Br4 Cu3 Cu4 57.19(3) 7_445 7_445
Cu6 Cu3 Cu4 120.63(2) . 7_445
Cu6 Cu3 Cu4 176.20(4) 4_445 7_445
Cu4 Cu3 Cu4 58.65(4) 4_445 7_445
O2 Cu3 Se3 71.2(2) . 7_445
O1 Cu3 Se3 110.75(19) 7_445 7_445
O7 Cu3 Se3 24.61(19) 7_445 7_445
O4 Cu3 Se3 149.79(19) . 7_445
Cu5 Cu3 Se3 107.69(5) . 7_445
Br4 Cu3 Se3 92.13(3) 7_435 7_445
Br4 Cu3 Se3 92.13(3) 7_445 7_445
Cu6 Cu3 Se3 60.76(3) . 7_445
Cu6 Cu3 Se3 60.76(3) 4_445 7_445
Cu4 Cu3 Se3 122.97(4) 4_445 7_445
Cu4 Cu3 Se3 122.97(4) 7_445 7_445
O1 Cu4 O3 176.6(3) . .
O1 Cu4 O6 85.8(2) . .
O3 Cu4 O6 96.2(2) . .
O1 Cu4 O8 98.4(2) . 7_445
O3 Cu4 O8 79.9(2) . 7_445
O6 Cu4 O8 171.59(19) . 7_445
O1 Cu4 Cu1 135.45(19) . .
O3 Cu4 Cu1 41.91(19) . .
O6 Cu4 Cu1 136.72(12) . .
O8 Cu4 Cu1 41.70(11) 7_445 .
O1 Cu4 Br5A 92.45(16) . .
O3 Cu4 Br5A 90.12(16) . .
O6 Cu4 Br5A 92.28(14) . .
O8 Cu4 Br5A 80.32(14) 7_445 .
Cu1 Cu4 Br5A 97.12(5) . .
O1 Cu4 Br4 90.44(17) . .
O3 Cu4 Br4 86.66(17) . .
O6 Cu4 Br4 97.44(13) . .
O8 Cu4 Br4 89.83(13) 7_445 .
Cu1 Cu4 Br4 74.26(4) . .
Br5A Cu4 Br4 170.04(6) . .
O1 Cu4 Cu4 35.51(16) . 6
O3 Cu4 Cu4 146.20(16) . 6
O6 Cu4 Cu4 97.66(12) . 6
O8 Cu4 Cu4 81.98(11) 7_445 6
Cu1 Cu4 Cu4 123.22(2) . 6
Br5A Cu4 Cu4 58.71(3) . 6
Br4 Cu4 Cu4 121.647(19) . 6
O1 Cu4 Cu3 34.13(18) . 7_445
O3 Cu4 Cu3 142.51(18) . 7_445
O6 Cu4 Cu3 105.71(13) . 7_445
O8 Cu4 Cu3 81.51(13) 7_445 7_445
Cu1 Cu4 Cu3 106.49(4) . 7_445
Br5A Cu4 Cu3 118.37(4) . 7_445
Br4 Cu4 Cu3 60.97(3) . 7_445
Cu4 Cu4 Cu3 60.676(19) 6 7_445
O1 Cu4 Cu4 144.49(16) . 6_545
O3 Cu4 Cu4 33.80(16) . 6_545
O6 Cu4 Cu4 82.34(12) . 6_545
O8 Cu4 Cu4 98.02(11) 7_445 6_545
Cu1 Cu4 Cu4 56.78(2) . 6_545
Br5A Cu4 Cu4 121.28(3) . 6_545
Br4 Cu4 Cu4 58.354(19) . 6_545
Cu4 Cu4 Cu4 180.0 6 6_545
Cu3 Cu4 Cu4 119.325(19) 7_445 6_545
O1 Cu4 Cu2 150.83(18) . .
O3 Cu4 Cu2 32.41(17) . .
O6 Cu4 Cu2 83.32(13) . .
O8 Cu4 Cu2 89.56(13) 7_445 .
Cu1 Cu4 Cu2 65.24(4) . .
Br5A Cu4 Cu2 61.12(3) . .
Br4 Cu4 Cu2 117.75(3) . .
Cu4 Cu4 Cu2 119.820(19) 6 .
Cu3 Cu4 Cu2 170.93(4) 7_445 .
Cu4 Cu4 Cu2 60.178(19) 6_545 .
O1 Cu4 Se1 110.71(18) . .
O3 Cu4 Se1 71.29(18) . .
O6 Cu4 Se1 24.93(12) . .
O8 Cu4 Se1 150.40(12) 7_445 .
Cu1 Cu4 Se1 112.13(3) . .
Br5A Cu4 Se1 92.77(5) . .
Br4 Cu4 Se1 95.12(3) . .
Cu4 Cu4 Se1 118.950(17) 6 .
Cu3 Cu4 Se1 126.12(4) 7_445 .
Cu4 Cu4 Se1 61.050(17) 6_545 .
Cu2 Cu4 Se1 62.35(3) . .
O2 Cu5 O4 76.6(3) . .
O2 Cu5 O9 78.57(16) . .
O4 Cu5 O9 113.62(14) . .
O2 Cu5 O9 78.57(16) . 6_545
O4 Cu5 O9 113.62(15) . 6_545
O9 Cu5 O9 120.0(3) . 6_545
O2 Cu5 Br3 180.0(2) . .
O4 Cu5 Br3 103.42(19) . .
O9 Cu5 Br3 101.41(13) . .
O9 Cu5 Br3 101.41(13) 6_545 .
O2 Cu5 Cu6 37.31(10) . 4_445
O4 Cu5 Cu6 96.56(16) . 4_445
O9 Cu5 Cu6 98.88(13) . 4_445
O9 Cu5 Cu6 41.30(13) 6_545 4_445
Br3 Cu5 Cu6 142.67(3) . 4_445
O2 Cu5 Cu6 37.31(10) . .
O4 Cu5 Cu6 96.56(16) . .
O9 Cu5 Cu6 41.30(13) . .
O9 Cu5 Cu6 98.88(13) 6_545 .
Br3 Cu5 Cu6 142.67(3) . .
Cu6 Cu5 Cu6 63.05(3) 4_445 .
O2 Cu5 Cu3 36.1(2) . .
O4 Cu5 Cu3 40.53(18) . .
O9 Cu5 Cu3 96.33(13) . .
O9 Cu5 Cu3 96.33(13) 6_545 .
Br3 Cu5 Cu3 143.95(6) . .
Cu6 Cu5 Cu3 62.48(3) 4_445 .
Cu6 Cu5 Cu3 62.48(3) . .
O2 Cu5 Se2 96.6(2) . .
O4 Cu5 Se2 19.96(18) . .
O9 Cu5 Se2 118.60(13) . .
O9 Cu5 Se2 118.60(13) 6_545 .
Br3 Cu5 Se2 83.46(5) . .
Cu6 Cu5 Se2 113.31(4) 4_445 .
Cu6 Cu5 Se2 113.31(4) . .
Cu3 Cu5 Se2 60.48(4) . .
O2 Cu5 Se3 95.82(10) . .
O4 Cu5 Se3 118.97(2) . .
O9 Cu5 Se3 17.26(13) . .
O9 Cu5 Se3 124.07(14) 6_545 .
Br3 Cu5 Se3 84.16(3) . .
Cu6 Cu5 Se3 113.13(4) 4_445 .
Cu6 Cu5 Se3 58.53(2) . .
Cu3 Cu5 Se3 111.16(3) . .
Se2 Cu5 Se3 117.33(2) . .
O2 Cu5 Se3 95.82(10) . 1_545
O4 Cu5 Se3 118.97(2) . 1_545
O9 Cu5 Se3 124.07(14) . 1_545
O9 Cu5 Se3 17.26(13) 6_545 1_545
Br3 Cu5 Se3 84.16(3) . 1_545
Cu6 Cu5 Se3 58.53(2) 4_445 1_545
Cu6 Cu5 Se3 113.13(4) . 1_545
Cu3 Cu5 Se3 111.16(3) . 1_545
Se2 Cu5 Se3 117.33(2) . 1_545
Se3 Cu5 Se3 122.04(5) . 1_545
O2 Cu5 Br4 56.38(11) . 7_435
O4 Cu5 Br4 55.73(10) . 7_435
O9 Cu5 Br4 134.74(13) . 7_435
O9 Cu5 Br4 59.15(13) 6_545 7_435
Br3 Cu5 Br4 123.64(3) . 7_435
Cu6 Cu5 Br4 47.89(2) 4_445 7_435
Cu6 Cu5 Br4 93.68(4) . 7_435
Cu3 Cu5 Br4 44.698(18) . 7_435
Se2 Cu5 Br4 67.62(3) . 7_435
Se3 Cu5 Br4 151.95(4) . 7_435
Se3 Cu5 Br4 69.72(3) 1_545 7_435
O2 Cu6 O2 180.0(4) 7_445 .
O2 Cu6 O9 82.5(2) 7_445 7_445
O2 Cu6 O9 97.5(2) . 7_445
O2 Cu6 O9 97.5(2) 7_445 .
O2 Cu6 O9 82.5(2) . .
O9 Cu6 O9 180.0 7_445 .
O2 Cu6 Cu5 141.99(19) 7_445 .
O2 Cu6 Cu5 38.01(19) . .
O9 Cu6 Cu5 135.50(12) 7_445 .
O9 Cu6 Cu5 44.50(12) . .
O2 Cu6 Cu5 38.01(19) 7_445 7_445
O2 Cu6 Cu5 141.99(19) . 7_445
O9 Cu6 Cu5 44.50(12) 7_445 7_445
O9 Cu6 Cu5 135.50(12) . 7_445
Cu5 Cu6 Cu5 180.0 . 7_445
O2 Cu6 Cu6 33.44(16) 7_445 4_455
O2 Cu6 Cu6 146.56(16) . 4_455
O9 Cu6 Cu6 97.45(12) 7_445 4_455
O9 Cu6 Cu6 82.55(12) . 4_455
Cu5 Cu6 Cu6 121.527(15) . 4_455
Cu5 Cu6 Cu6 58.474(15) 7_445 4_455
O2 Cu6 Cu6 146.56(16) 7_445 4_445
O2 Cu6 Cu6 33.44(16) . 4_445
O9 Cu6 Cu6 82.55(12) 7_445 4_445
O9 Cu6 Cu6 97.45(12) . 4_445
Cu5 Cu6 Cu6 58.473(15) . 4_445
Cu5 Cu6 Cu6 121.526(15) 7_445 4_445
Cu6 Cu6 Cu6 180.0 4_455 4_445
O2 Cu6 Cu3 33.63(18) 7_445 7_445
O2 Cu6 Cu3 146.37(18) . 7_445
O9 Cu6 Cu3 96.56(14) 7_445 7_445
O9 Cu6 Cu3 83.44(14) . 7_445
Cu5 Cu6 Cu3 120.22(3) . 7_445
Cu5 Cu6 Cu3 59.78(3) 7_445 7_445
Cu6 Cu6 Cu3 60.094(14) 4_455 7_445
Cu6 Cu6 Cu3 119.906(14) 4_445 7_445
O2 Cu6 Cu3 146.37(18) 7_445 .
O2 Cu6 Cu3 33.63(18) . .
O9 Cu6 Cu3 83.44(14) 7_445 .
O9 Cu6 Cu3 96.56(14) . .
Cu5 Cu6 Cu3 59.78(3) . .
Cu5 Cu6 Cu3 120.22(3) 7_445 .
Cu6 Cu6 Cu3 119.906(14) 4_455 .
Cu6 Cu6 Cu3 60.094(14) 4_445 .
Cu3 Cu6 Cu3 180.0 7_445 .
O2 Cu6 Se3 107.74(19) 7_445 7_445
O2 Cu6 Se3 72.26(19) . 7_445
O9 Cu6 Se3 25.29(12) 7_445 7_445
O9 Cu6 Se3 154.71(12) . 7_445
Cu5 Cu6 Se3 110.23(3) . 7_445
Cu5 Cu6 Se3 69.76(3) 7_445 7_445
Cu6 Cu6 Se3 118.762(12) 4_455 7_445
Cu6 Cu6 Se3 61.238(12) 4_445 7_445
Cu3 Cu6 Se3 118.13(3) 7_445 7_445
Cu3 Cu6 Se3 61.87(3) . 7_445
O2 Cu6 Se3 72.26(19) 7_445 .
O2 Cu6 Se3 107.74(19) . .
O9 Cu6 Se3 154.71(12) 7_445 .
O9 Cu6 Se3 25.29(12) . .
Cu5 Cu6 Se3 69.76(3) . .
Cu5 Cu6 Se3 110.24(3) 7_445 .
Cu6 Cu6 Se3 61.238(12) 4_455 .
Cu6 Cu6 Se3 118.762(12) 4_445 .
Cu3 Cu6 Se3 61.87(3) 7_445 .
Cu3 Cu6 Se3 118.13(3) . .
Se3 Cu6 Se3 180.0 7_445 .
Br5B Br5A Cu7 103.3(18) . .
Br5B Br5A Cu7 103.3(18) . 6
Cu7 Br5A Cu7 26.45(14) . 6
Br5B Br5A Br5B 23(2) . 5_556
Cu7 Br5A Br5B 125.3(3) . 5_556
Cu7 Br5A Br5B 125.3(3) 6 5_556
Br5B Br5A Cu4 131.2(13) . 6
Cu7 Br5A Cu4 118.82(11) . 6
Cu7 Br5A Cu4 104.15(9) 6 6
Br5B Br5A Cu4 113.4(2) 5_556 6
Br5B Br5A Cu4 131.2(13) . .
Cu7 Br5A Cu4 104.15(10) . .
Cu7 Br5A Cu4 118.82(11) 6 .
Br5B Br5A Cu4 113.4(2) 5_556 .
Cu4 Br5A Cu4 62.57(5) 6 .
Br5B Br5A Cu2 86.29(7) . .
Cu7 Br5A Cu2 76.20(8) . .
Cu7 Br5A Cu2 102.59(9) 6 .
Br5B Br5A Cu2 87.17(5) 5_556 .
Cu4 Br5A Cu2 125.11(6) 6 .
Cu4 Br5A Cu2 62.56(3) . .
Br5B Br5A Cu2 86.29(7) . 1_565
Cu7 Br5A Cu2 102.58(9) . 1_565
Cu7 Br5A Cu2 76.19(8) 6 1_565
Br5B Br5A Cu2 87.17(6) 5_556 1_565
Cu4 Br5A Cu2 62.56(3) 6 1_565
Cu4 Br5A Cu2 125.11(6) . 1_565
Cu2 Br5A Cu2 171.98(9) . 1_565
Br5B Br5A O8 157.49(11) . 7_445
Cu7 Br5A O8 71.56(12) . 7_445
Cu7 Br5A O8 81.88(13) 6 7_445
Br5B Br5A O8 149.19(18) 5_556 7_445
Cu4 Br5A O8 66.37(9) 6 7_445
Cu4 Br5A O8 37.06(8) . 7_445
Cu2 Br5A O8 71.21(8) . 7_445
Cu2 Br5A O8 116.15(9) 1_565 7_445
Br5B Br5A O8 157.49(12) . 4_455
Cu7 Br5A O8 81.88(13) . 4_455
Cu7 Br5A O8 71.56(12) 6 4_455
Br5B Br5A O8 149.19(18) 5_556 4_455
Cu4 Br5A O8 37.06(8) 6 4_455
Cu4 Br5A O8 66.37(9) . 4_455
Cu2 Br5A O8 116.15(9) . 4_455
Cu2 Br5A O8 71.21(8) 1_565 4_455
O8 Br5A O8 44.97(14) 7_445 4_455
Br5B Br5A Br5A 19.5(18) . 5_556
Cu7 Br5A Br5A 122.15(12) . 5_556
Cu7 Br5A Br5A 122.15(12) 6 5_556
Br5B Br5A Br5A 3.2(3) 5_556 5_556
Cu4 Br5A Br5A 116.09(8) 6 5_556
Cu4 Br5A Br5A 116.09(8) . 5_556
Cu2 Br5A Br5A 87.01(5) . 5_556
Cu2 Br5A Br5A 87.01(5) 1_565 5_556
O8 Br5A Br5A 151.25(9) 7_445 5_556
O8 Br5A Br5A 151.25(9) 4_455 5_556
Br5B Br5A O3 115.4(4) . 1_565
Cu7 Br5A O3 106.32(14) . 1_565
Cu7 Br5A O3 82.91(13) 6 1_565
Br5B Br5A O3 108.83(13) 5_556 1_565
Cu4 Br5A O3 32.51(9) 6 1_565
Cu4 Br5A O3 94.29(11) . 1_565
Cu2 Br5A O3 156.13(12) . 1_565
Cu2 Br5A O3 31.89(9) 1_565 1_565
O8 Br5A O3 86.88(12) 7_445 1_565
O8 Br5A O3 43.07(11) 4_455 1_565
Br5A Br5A O3 109.96(10) 5_556 1_565
Br5A Br5B Cu7 65.4(17) . .
Br5A Br5B Cu7 65.4(17) . 6
Cu7 Br5B Cu7 24.69(19) . 6
Br5A Br5B Br5B 153(2) . 5_556
Cu7 Br5B Br5B 140.7(9) . 5_556
Cu7 Br5B Br5B 140.7(9) 6 5_556
Br5A Br5B Br5A 157(2) . 5_556
Cu7 Br5B Br5A 136.5(5) . 5_556
Cu7 Br5B Br5A 136.5(5) 6 5_556
Br5B Br5B Br5A 4.4(4) 5_556 5_556
Br5A Br5B Cu2 84.6(2) . .
Cu7 Br5B Cu2 74.0(2) . .
Cu7 Br5B Cu2 98.6(3) 6 .
Br5B Br5B Cu2 95.5(2) 5_556 .
Br5A Br5B Cu2 95.6(2) 5_556 .
Br5A Br5B Cu2 84.6(2) . 1_565
Cu7 Br5B Cu2 98.6(3) . 1_565
Cu7 Br5B Cu2 74.0(2) 6 1_565
Br5B Br5B Cu2 95.5(2) 5_556 1_565
Br5A Br5B Cu2 95.6(2) 5_556 1_565
Cu2 Br5B Cu2 168.7(5) . 1_565
Br5A Br5B Cu4 42.3(12) . 6
Cu7 Br5B Cu4 102.8(4) . 6
Cu7 Br5B Cu4 91.3(3) 6 6
Br5B Br5B Cu4 115.8(7) 5_556 6
Br5A Br5B Cu4 119.6(4) 5_556 6
Cu2 Br5B Cu4 113.9(3) . 6
Cu2 Br5B Cu4 58.71(14) 1_565 6
Br5A Br5B Cu4 42.3(12) . .
Cu7 Br5B Cu4 91.3(3) . .
Cu7 Br5B Cu4 102.8(4) 6 .
Br5B Br5B Cu4 115.8(7) 5_556 .
Br5A Br5B Cu4 119.6(4) 5_556 .
Cu2 Br5B Cu4 58.71(14) . .
Cu2 Br5B Cu4 113.9(3) 1_565 .
Cu4 Br5B Cu4 55.4(2) 6 .
Br5A Br5B O5 116.6(4) . 5_556
Cu7 Br5B O5 103.7(4) . 5_556
Cu7 Br5B O5 82.0(3) 6 5_556
Br5B Br5B O5 70.9(3) 5_556 5_556
Br5A Br5B O5 69.4(2) 5_556 5_556
Cu2 Br5B O5 156.2(4) . 5_556
Cu2 Br5B O5 33.04(11) 1_565 5_556
Cu4 Br5B O5 89.85(13) 6 5_556
Cu4 Br5B O5 144.7(3) . 5_556
Br5A Br5B O5 116.6(4) . 5_546
Cu7 Br5B O5 82.0(3) . 5_546
Cu7 Br5B O5 103.7(4) 6 5_546
Br5B Br5B O5 70.9(3) 5_556 5_546
Br5A Br5B O5 69.4(2) 5_556 5_546
Cu2 Br5B O5 33.04(11) . 5_546
Cu2 Br5B O5 156.2(4) 1_565 5_546
Cu4 Br5B O5 144.7(3) 6 5_546
Cu4 Br5B O5 89.85(13) . 5_546
O5 Br5B O5 123.5(4) 5_556 5_546
Br5A Br5B O5 100.0(9) . 1_565
Cu7 Br5B O5 132.2(3) . 1_565
Cu7 Br5B O5 107.53(17) 6 1_565
Br5B Br5B O5 68.4(3) 5_556 1_565
Br5A Br5B O5 70.0(2) 5_556 1_565
Cu2 Br5B O5 153.0(5) . 1_565
Cu2 Br5B O5 33.58(11) 1_565 1_565
Cu4 Br5B O5 59.91(18) 6 1_565
Cu4 Br5B O5 107.7(4) . 1_565
O5 Br5B O5 39.8(2) 5_556 1_565
O5 Br5B O5 139.3(4) 5_546 1_565
Cu7 Cu7 Br5A 76.77(7) 6 .
Cu7 Cu7 Br5B 77.65(10) 6 .
Br5A Cu7 Br5B 11.3(3) . .
Cu7 Cu7 Br2 77.75(6) 6 7_446
Br5A Cu7 Br2 108.97(13) . 7_446
Br5B Cu7 Br2 98.4(3) . 7_446
Cu7 Cu7 Br1 77.81(6) 6 7_446
Br5A Cu7 Br1 127.45(13) . 7_446
Br5B Cu7 Br1 137.6(3) . 7_446
Br2 Cu7 Br1 109.42(11) 7_446 7_446
Cu7 Cu7 Br1 175.12(7) 6 .
Br5A Cu7 Br1 107.26(11) . .
Br5B Cu7 Br1 106.85(13) . .
Br2 Cu7 Br1 103.11(10) 7_446 .
Br1 Cu7 Br1 97.43(10) 7_446 .
Cu7 Cu7 Cu1 80.10(5) 6 7_446
Br5A Cu7 Cu1 151.01(12) . 7_446
Br5B Cu7 Cu1 143.5(3) . 7_446
Br2 Cu7 Cu1 48.34(6) 7_446 7_446
Br1 Cu7 Cu1 62.71(7) 7_446 7_446
Br1 Cu7 Cu1 96.84(9) . 7_446
Cu7 Cu7 Cu7 127.58(10) 6 7_446
Br5A Cu7 Cu7 132.97(16) . 7_446
Br5B Cu7 Cu7 140.7(3) . 7_446
Br2 Cu7 Cu7 114.99(13) 7_446 7_446
Br1 Cu7 Cu7 49.78(8) 7_446 7_446
Br1 Cu7 Cu7 47.65(7) . 7_446
Cu1 Cu7 Cu7 75.52(10) 7_446 7_446
Cu7 Cu7 O8 102.49(8) 6 7_445
Br5A Cu7 O8 67.81(11) . 7_445
Br5B Cu7 O8 78.3(3) . 7_445
Br2 Cu7 O8 176.50(14) 7_446 7_445
Br1 Cu7 O8 73.99(10) 7_446 7_445
Br1 Cu7 O8 76.96(10) . 7_445
Cu1 Cu7 O8 135.16(13) 7_446 7_445
Cu7 Cu7 O8 67.71(11) 7_446 7_445
Cu7 Cu7 Cu2 139.18(5) 6 .
Br5A Cu7 Cu2 62.60(7) . .
Br5B Cu7 Cu2 61.76(10) . .
Br2 Cu7 Cu2 110.70(11) 7_446 .
Br1 Cu7 Cu2 130.03(10) 7_446 .
Br1 Cu7 Cu2 45.16(5) . .
Cu1 Cu7 Cu2 136.23(9) 7_446 .
Cu7 Cu7 Cu2 86.35(11) 7_446 .
O8 Cu7 Cu2 66.80(9) 7_445 .
Cu7 Cu7 Br1 3.46(5) 6 1_565
Br5A Cu7 Br1 79.66(7) . 1_565
Br5B Cu7 Br1 80.86(10) . 1_565
Br2 Cu7 Br1 78.41(7) 7_446 1_565
Br1 Cu7 Br1 74.43(7) 7_446 1_565
Br1 Cu7 Br1 171.66(12) . 1_565
Cu1 Cu7 Br1 77.95(6) 7_446 1_565
Cu7 Cu7 Br1 124.19(14) 7_446 1_565
O8 Cu7 Br1 102.04(10) 7_445 1_565
Cu2 Cu7 Br1 142.20(9) . 1_565
Cu7 Cu7 O8 61.49(7) 6 4_455
Br5A Cu7 O8 60.42(10) . 4_455
Br5B Cu7 O8 70.9(3) . 4_455
Br2 Cu7 O8 139.09(11) 7_446 4_455
Br1 Cu7 O8 67.04(9) 7_446 4_455
Br1 Cu7 O8 117.80(11) . 4_455
Cu1 Cu7 O8 121.51(11) 7_446 4_455
Cu7 Cu7 O8 93.92(13) 7_446 4_455
O8 Cu7 O8 40.99(13) 7_445 4_455
Cu2 Cu7 O8 98.85(10) . 4_455
Br1 Cu7 O8 61.12(8) 1_565 4_455
Cu4 O1 Cu4 109.0(3) . 6
Cu4 O1 Cu3 112.0(2) . 7_445
Cu4 O1 Cu3 112.0(2) 6 7_445
Cu4 O1 Pb1 107.8(2) . .
Cu4 O1 Pb1 107.8(2) 6 .
Cu3 O1 Pb1 108.2(3) 7_445 .
Cu4 O1 O6 48.15(14) . .
Cu4 O1 O6 116.8(3) 6 .
Cu3 O1 O6 131.12(18) 7_445 .
Pb1 O1 O6 59.99(16) . .
Cu4 O1 O6 116.8(3) . 6
Cu4 O1 O6 48.15(14) 6 6
Cu3 O1 O6 131.12(18) 7_445 6
Pb1 O1 O6 59.99(16) . 6
O6 O1 O6 86.7(3) . 6
Cu4 O1 O7 125.49(16) . .
Cu4 O1 O7 125.49(16) 6 .
Cu3 O1 O7 48.3(2) 7_445 .
Pb1 O1 O7 60.0(2) . .
O6 O1 O7 101.9(2) . .
O6 O1 O7 101.9(2) 6 .
Cu4 O1 O8 42.35(14) . 7_445
Cu4 O1 O8 87.4(2) 6 7_445
Cu3 O1 O8 88.5(2) 7_445 7_445
Pb1 O1 O8 150.11(17) . 7_445
O6 O1 O8 90.26(17) . 7_445
O6 O1 O8 126.1(3) 6 7_445
O7 O1 O8 131.1(2) . 7_445
Cu4 O1 O8 87.4(2) . 4_455
Cu4 O1 O8 42.35(14) 6 4_455
Cu3 O1 O8 88.5(2) 7_445 4_455
Pb1 O1 O8 150.11(17) . 4_455
O6 O1 O8 126.1(3) . 4_455
O6 O1 O8 90.26(17) 6 4_455
O7 O1 O8 131.1(2) . 4_455
O8 O1 O8 50.41(18) 7_445 4_455
Cu4 O1 O4 89.2(2) . 7_445
Cu4 O1 O4 89.2(2) 6 7_445
Cu3 O1 O4 41.40(18) 7_445 7_445
Pb1 O1 O4 149.7(3) . 7_445
O6 O1 O4 134.28(15) . 7_445
O6 O1 O4 134.28(15) 6 7_445
O7 O1 O4 89.7(3) . 7_445
O8 O1 O4 51.88(17) 7_445 7_445
O8 O1 O4 51.88(17) 4_455 7_445
Cu4 O1 Se2 72.51(18) . 7_445
Cu4 O1 Se2 72.51(18) 6 7_445
Cu3 O1 Se2 71.23(18) 7_445 7_445
Pb1 O1 Se2 179.5(3) . 7_445
O6 O1 Se2 120.33(18) . 7_445
O6 O1 Se2 120.33(18) 6 7_445
O7 O1 Se2 119.5(2) . 7_445
O8 O1 Se2 30.17(10) 7_445 7_445
O8 O1 Se2 30.17(10) 4_455 7_445
O4 O1 Se2 29.83(14) 7_445 7_445
Cu4 O1 Br4 57.43(9) . .
Cu4 O1 Br4 152.4(3) 6 .
Cu3 O1 Br4 61.07(9) 7_445 .
Pb1 O1 Br4 99.56(13) . .
O6 O1 Br4 73.86(10) . .
O6 O1 Br4 157.5(2) 6 .
O7 O1 Br4 71.91(12) . .
O8 O1 Br4 66.48(11) 7_445 .
O8 O1 Br4 110.26(18) 4_455 .
O4 O1 Br4 68.10(10) 7_445 .
Se2 O1 Br4 80.20(10) 7_445 .
Cu6 O2 Cu6 113.1(3) . 4_445
Cu6 O2 Cu3 113.0(2) . .
Cu6 O2 Cu3 113.0(2) 4_445 .
Cu6 O2 Cu5 104.7(2) . .
Cu6 O2 Cu5 104.7(2) 4_445 .
Cu3 O2 Cu5 107.4(3) . .
Cu6 O2 O4 123.07(16) . .
Cu6 O2 O4 123.07(16) 4_445 .
Cu3 O2 O4 52.8(2) . .
Cu5 O2 O4 54.6(2) . .
Cu6 O2 O9 124.1(3) . 6_545
Cu6 O2 O9 50.56(14) 4_445 6_545
Cu3 O2 O9 122.5(2) . 6_545
Cu5 O2 O9 54.18(17) . 6_545
O4 O2 O9 88.3(2) . 6_545
Cu6 O2 O9 50.56(14) . .
Cu6 O2 O9 124.1(3) 4_445 .
Cu3 O2 O9 122.5(2) . .
Cu5 O2 O9 54.18(17) . .
O4 O2 O9 88.3(2) . .
O9 O2 O9 91.5(3) 6_545 .
Cu6 O2 O7 90.9(2) . 7_445
Cu6 O2 O7 90.9(2) 4_445 7_445
Cu3 O2 O7 43.54(19) . 7_445
Cu5 O2 O7 151.0(3) . 7_445
O4 O2 O7 96.3(3) . 7_445
O9 O2 O7 134.11(15) 6_545 7_445
O9 O2 O7 134.11(15) . 7_445
Cu6 O2 O9 91.0(2) . 4_445
Cu6 O2 O9 42.60(15) 4_445 4_445
Cu3 O2 O9 91.9(2) . 4_445
Cu5 O2 O9 147.2(2) . 4_445
O4 O2 O9 137.0(3) . 4_445
O9 O2 O9 93.16(17) 6_545 4_445
O9 O2 O9 134.5(3) . 4_445
O7 O2 O9 53.86(18) 7_445 4_445
Cu6 O2 O9 42.60(15) . 7_445
Cu6 O2 O9 91.0(2) 4_445 7_445
Cu3 O2 O9 91.9(2) . 7_445
Cu5 O2 O9 147.2(2) . 7_445
O4 O2 O9 137.0(3) . 7_445
O9 O2 O9 134.5(3) 6_545 7_445
O9 O2 O9 93.16(17) . 7_445
O7 O2 O9 53.86(18) 7_445 7_445
O9 O2 O9 53.6(2) 4_445 7_445
Cu6 O2 Se3 74.07(19) . 7_445
Cu6 O2 Se3 74.07(19) 4_445 7_445
Cu3 O2 Se3 75.0(2) . 7_445
Cu5 O2 Se3 177.5(3) . 7_445
O4 O2 Se3 127.8(3) . 7_445
O9 O2 Se3 124.62(18) 6_545 7_445
O9 O2 Se3 124.62(18) . 7_445
O7 O2 Se3 31.51(15) 7_445 7_445
O9 O2 Se3 31.47(11) 4_445 7_445
O9 O2 Se3 31.47(11) 7_445 7_445
Cu6 O2 O2 0.0 . 7_445
Cu6 O2 O2 113.1(3) 4_445 7_445
Cu3 O2 O2 113.0(2) . 7_445
Cu5 O2 O2 104.7(2) . 7_445
O4 O2 O2 123.07(16) . 7_445
O9 O2 O2 124.1(3) 6_545 7_445
O9 O2 O2 50.56(14) . 7_445
O7 O2 O2 90.9(2) 7_445 7_445
O9 O2 O2 91.0(2) 4_445 7_445
O9 O2 O2 42.60(15) 7_445 7_445
Se3 O2 O2 74.07(19) 7_445 7_445
Cu2 O3 Cu4 114.6(2) . 6_545
Cu2 O3 Cu4 114.6(2) . .
Cu4 O3 Cu4 112.4(3) 6_545 .
Cu2 O3 Cu1 118.4(3) . .
Cu4 O3 Cu1 97.2(2) 6_545 .
Cu4 O3 Cu1 97.2(2) . .
Cu2 O3 O8 116.5(2) . 4_445
Cu4 O3 O8 52.15(13) 6_545 4_445
Cu4 O3 O8 127.9(3) . 4_445
Cu1 O3 O8 48.95(14) . 4_445
Cu2 O3 O8 116.5(2) . 7_445
Cu4 O3 O8 127.9(3) 6_545 7_445
Cu4 O3 O8 52.15(13) . 7_445
Cu1 O3 O8 48.95(14) . 7_445
O8 O3 O8 95.2(3) 4_445 7_445
Cu2 O3 O5 44.71(19) . .
Cu4 O3 O5 92.1(2) 6_545 .
Cu4 O3 O5 92.1(2) . .
Cu1 O3 O5 163.1(3) . .
O8 O3 O5 132.28(14) 4_445 .
O8 O3 O5 132.28(14) 7_445 .
Cu2 O3 O6 93.7(2) . 6_545
Cu4 O3 O6 42.78(14) 6_545 6_545
Cu4 O3 O6 91.5(2) . 6_545
Cu1 O3 O6 138.5(2) . 6_545
O8 O3 O6 94.66(16) 4_445 6_545
O8 O3 O6 139.2(3) 7_445 6_545
O5 O3 O6 54.72(17) . 6_545
Cu2 O3 O6 93.7(2) . .
Cu4 O3 O6 91.5(2) 6_545 .
Cu4 O3 O6 42.78(15) . .
Cu1 O3 O6 138.5(2) . .
O8 O3 O6 139.2(3) 4_445 .
O8 O3 O6 94.66(16) 7_445 .
O5 O3 O6 54.72(17) . .
O6 O3 O6 54.4(2) 6_545 .
Cu2 O3 Br1 51.33(15) . .
Cu4 O3 Br1 123.23(16) 6_545 .
Cu4 O3 Br1 123.23(16) . .
Cu1 O3 Br1 67.02(18) . .
O8 O3 Br1 83.36(19) 4_445 .
O8 O3 Br1 83.36(19) 7_445 .
O5 O3 Br1 96.0(2) . .
O6 O3 Br1 137.15(19) 6_545 .
O6 O3 Br1 137.15(19) . .
Cu2 O3 Se1 77.1(2) . .
Cu4 O3 Se1 74.55(18) 6_545 .
Cu4 O3 Se1 74.55(18) . .
Cu1 O3 Se1 164.5(3) . .
O8 O3 Se1 126.30(17) 4_445 .
O8 O3 Se1 126.30(17) 7_445 .
O5 O3 Se1 32.44(15) . .
O6 O3 Se1 31.77(10) 6_545 .
O6 O3 Se1 31.77(10) . .
Br1 O3 Se1 128.5(2) . .
Cu2 O3 Br4 165.0(3) . .
Cu4 O3 Br4 60.14(16) 6_545 .
Cu4 O3 Br4 60.14(16) . .
Cu1 O3 Br4 76.63(19) . .
O8 O3 Br4 72.51(18) 4_445 .
O8 O3 Br4 72.51(18) 7_445 .
O5 O3 Br4 120.3(2) . .
O6 O3 Br4 73.01(16) 6_545 .
O6 O3 Br4 73.00(16) . .
Br1 O3 Br4 143.7(2) . .
Se1 O3 Br4 87.87(15) . .
Se2 O4 Cu3 127.3(4) . .
Se2 O4 Cu5 135.3(4) . .
Cu3 O4 Cu5 97.4(3) . .
Se2 O4 O2 176.0(4) . .
Cu3 O4 O2 48.6(2) . .
Cu5 O4 O2 48.7(2) . .
Se2 O4 O8 39.86(15) . .
Cu3 O4 O8 97.6(2) . .
Cu5 O4 O8 147.13(18) . .
O2 O4 O8 137.4(2) . .
Se2 O4 O8 39.86(15) . 6_545
Cu3 O4 O8 97.6(2) . 6_545
Cu5 O4 O8 147.13(18) . 6_545
O2 O4 O8 137.4(2) . 6_545
O8 O4 O8 58.1(2) . 6_545
Se2 O4 O1 88.2(3) . 7_445
Cu3 O4 O1 39.14(17) . 7_445
Cu5 O4 O1 136.5(3) . 7_445
O2 O4 O1 87.8(3) . 7_445
O8 O4 O1 63.7(2) . 7_445
O8 O4 O1 63.7(2) 6_545 7_445
Se2 O4 Br3 94.2(2) . .
Cu3 O4 Br3 138.5(3) . .
Cu5 O4 Br3 41.12(13) . .
O2 O4 Br3 89.9(2) . .
O8 O4 Br3 118.2(2) . .
O8 O4 Br3 118.2(2) 6_545 .
O1 O4 Br3 177.6(3) 7_445 .
Se2 O4 O9 136.0(2) . .
Cu3 O4 O9 85.9(2) . .
Cu5 O4 O9 33.51(10) . .
O2 O4 O9 46.73(16) . .
O8 O4 O9 119.38(11) . .
O8 O4 O9 175.8(2) 6_545 .
O1 O4 O9 118.7(2) 7_445 .
Br3 O4 O9 59.37(13) . .
Se2 O4 O9 136.0(2) . 6_545
Cu3 O4 O9 85.9(2) . 6_545
Cu5 O4 O9 33.51(10) . 6_545
O2 O4 O9 46.73(16) . 6_545
O8 O4 O9 175.8(2) . 6_545
O8 O4 O9 119.38(11) 6_545 6_545
O1 O4 O9 118.7(2) 7_445 6_545
Br3 O4 O9 59.37(13) . 6_545
O9 O4 O9 62.92(18) . 6_545
Se2 O4 Cu4 70.13(19) . 4_445
Cu3 O4 Cu4 62.95(16) . 4_445
Cu5 O4 Cu4 145.74(18) . 4_445
O2 O4 Cu4 106.3(2) . 4_445
O8 O4 Cu4 66.71(17) . 4_445
O8 O4 Cu4 34.68(12) 6_545 4_445
O1 O4 Cu4 32.70(9) 7_445 4_445
Br3 O4 Cu4 148.62(12) . 4_445
O9 O4 Cu4 148.8(2) . 4_445
O9 O4 Cu4 113.34(11) 6_545 4_445
Se2 O4 Cu4 70.13(19) . 7_445
Cu3 O4 Cu4 62.95(16) . 7_445
Cu5 O4 Cu4 145.74(18) . 7_445
O2 O4 Cu4 106.3(2) . 7_445
O8 O4 Cu4 34.68(12) . 7_445
O8 O4 Cu4 66.71(17) 6_545 7_445
O1 O4 Cu4 32.70(9) 7_445 7_445
Br3 O4 Cu4 148.62(12) . 7_445
O9 O4 Cu4 113.34(11) . 7_445
O9 O4 Cu4 148.8(2) 6_545 7_445
Cu4 O4 Cu4 52.18(10) 4_445 7_445
Se1 O5 Cu2 129.5(4) . 5_546
Se1 O5 Cu2 126.9(4) . .
Cu2 O5 Cu2 103.6(3) 5_546 .
Se1 O5 O5 177.6(5) . 5_546
Cu2 O5 O5 52.9(2) 5_546 5_546
Cu2 O5 O5 50.7(2) . 5_546
Se1 O5 O6 39.40(14) . 6_545
Cu2 O5 O6 142.4(2) 5_546 6_545
Cu2 O5 O6 98.7(2) . 6_545
O5 O5 O6 139.1(3) 5_546 6_545
Se1 O5 O6 39.40(14) . .
Cu2 O5 O6 142.4(2) 5_546 .
Cu2 O5 O6 98.7(2) . .
O5 O5 O6 139.1(3) 5_546 .
O6 O5 O6 60.2(2) 6_545 .
Se1 O5 O3 85.7(3) . .
Cu2 O5 O3 144.8(3) 5_546 .
Cu2 O5 O3 41.19(18) . .
O5 O5 O3 91.9(4) 5_546 .
O6 O5 O3 63.48(19) 6_545 .
O6 O5 O3 63.48(19) . .
Se1 O5 Br1 82.7(2) . 5_546
Cu2 O5 Br1 46.78(15) 5_546 5_546
Cu2 O5 Br1 150.4(3) . 5_546
O5 O5 Br1 99.7(3) 5_546 5_546
O6 O5 Br1 106.8(2) 6_545 5_546
O6 O5 Br1 106.8(2) . 5_546
O3 O5 Br1 168.4(3) . 5_546
Se1 O5 Cu4 68.52(18) . 6_545
Cu2 O5 Cu4 149.24(14) 5_546 6_545
Cu2 O5 Cu4 64.54(16) . 6_545
O5 O5 Cu4 109.4(3) 5_546 6_545
O6 O5 Cu4 34.21(12) 6_545 6_545
O6 O5 Cu4 68.23(16) . 6_545
O3 O5 Cu4 33.16(9) . 6_545
Br1 O5 Cu4 139.37(16) 5_546 6_545
Se1 O5 Cu4 68.52(18) . .
Cu2 O5 Cu4 149.24(14) 5_546 .
Cu2 O5 Cu4 64.54(16) . .
O5 O5 Cu4 109.4(3) 5_546 .
O6 O5 Cu4 68.23(16) 6_545 .
O6 O5 Cu4 34.21(12) . .
O3 O5 Cu4 33.16(9) . .
Br1 O5 Cu4 139.37(16) 5_546 .
Cu4 O5 Cu4 54.11(10) 6_545 .
Se1 O5 Br5B 109.5(3) . 5_556
Cu2 O5 Br5B 61.9(2) 5_546 5_556
Cu2 O5 Br5B 94.0(3) . 5_556
O5 O5 Br5B 71.4(3) 5_546 5_556
O6 O5 Br5B 146.1(3) 6_545 5_556
O6 O5 Br5B 87.0(2) . 5_556
O3 O5 Br5B 111.1(2) . 5_556
Br1 O5 Br5B 73.0(2) 5_546 5_556
Cu4 O5 Br5B 142.7(2) 6_545 5_556
Cu4 O5 Br5B 89.69(19) . 5_556
Se1 O5 Br5B 109.5(3) . 5_546
Cu2 O5 Br5B 61.9(2) 5_546 5_546
Cu2 O5 Br5B 94.0(3) . 5_546
O5 O5 Br5B 71.4(3) 5_546 5_546
O6 O5 Br5B 87.0(2) 6_545 5_546
O6 O5 Br5B 146.1(3) . 5_546
O3 O5 Br5B 111.1(2) . 5_546
Br1 O5 Br5B 73.0(2) 5_546 5_546
Cu4 O5 Br5B 89.69(19) 6_545 5_546
Cu4 O5 Br5B 142.7(2) . 5_546
Br5B O5 Br5B 123.5(4) 5_556 5_546
Se1 O6 Cu4 125.8(2) . .
Se1 O6 Pb1 135.1(2) . .
Cu4 O6 Pb1 97.99(16) . .
Se1 O6 O5 40.22(15) . .
Cu4 O6 O5 97.1(2) . .
Pb1 O6 O5 154.6(2) . .
Se1 O6 O1 171.3(3) . .
Cu4 O6 O1 46.00(15) . .
Pb1 O6 O1 52.31(15) . .
O5 O6 O1 136.3(3) . .
Se1 O6 O6 39.02(15) . 6_545
Cu4 O6 O6 97.66(12) . 6_545
Pb1 O6 O6 137.19(10) . 6_545
O5 O6 O6 59.91(11) . 6_545
O1 O6 O6 133.37(13) . 6_545
Se1 O6 O3 84.80(18) . .
Cu4 O6 O3 41.01(12) . .
Pb1 O6 O3 138.3(2) . .
O5 O6 O3 61.8(2) . .
O1 O6 O3 86.98(19) . .
O6 O6 O3 62.78(10) 6_545 .
Se1 O6 Cu4 68.08(13) . 6_545
Cu4 O6 Cu4 63.71(11) . 6_545
Pb1 O6 Cu4 137.90(16) . 6_545
O5 O6 Cu4 67.45(14) . 6_545
O1 O6 Cu4 103.29(16) . 6_545
O6 O6 Cu4 33.95(7) 6_545 6_545
O3 O6 Cu4 32.96(8) . 6_545
Se1 O6 Br2 85.21(16) . 3
Cu4 O6 Br2 139.20(18) . 3
Pb1 O6 Br2 63.18(9) . 3
O5 O6 Br2 92.22(17) . 3
O1 O6 Br2 103.40(16) . 3
O6 O6 Br2 121.06(7) 6_545 3
O3 O6 Br2 148.7(2) . 3
Cu4 O6 Br2 153.29(13) 6_545 3
Se1 O6 Br3 76.67(15) . 5_545
Cu4 O6 Br3 124.04(18) . 5_545
Pb1 O6 Br3 70.10(11) . 5_545
O5 O6 Br3 116.72(17) . 5_545
O1 O6 Br3 105.21(19) . 5_545
O6 O6 Br3 68.10(7) 6_545 5_545
O3 O6 Br3 120.86(16) . 5_545
Cu4 O6 Br3 88.73(10) 6_545 5_545
Br2 O6 Br3 85.25(10) 3 5_545
Se1 O6 Cu2 69.19(14) . .
Cu4 O6 Cu2 63.14(12) . .
Pb1 O6 Cu2 152.76(16) . .
O5 O6 Cu2 34.00(15) . .
O1 O6 Cu2 104.91(19) . .
O6 O6 Cu2 68.13(7) 6_545 .
O3 O6 Cu2 31.91(13) . .
Cu4 O6 Cu2 53.73(7) 6_545 .
Br2 O6 Cu2 117.33(12) 3 .
Br3 O6 Cu2 136.22(12) 5_545 .
Se1 O6 O6 140.98(15) . 6
Cu4 O6 O6 82.34(12) . 6
Pb1 O6 O6 42.81(10) . 6
O5 O6 O6 120.09(11) . 6
O1 O6 O6 46.63(13) . 6
O6 O6 O6 180.0 6_545 6
O3 O6 O6 117.22(10) . 6
Cu4 O6 O6 146.05(7) 6_545 6
Br2 O6 O6 58.94(7) 3 6
Br3 O6 O6 111.91(7) 5_545 6
Cu2 O6 O6 111.87(7) . 6
Se3 O7 Cu3 125.9(4) . 7_445
Se3 O7 Pb1 136.8(3) . .
Cu3 O7 Pb1 97.3(3) 7_445 .
Se3 O7 O9 39.11(15) . .
Cu3 O7 O9 98.2(2) 7_445 .
Pb1 O7 O9 146.07(17) . .
Se3 O7 O9 39.11(15) . 6
Cu3 O7 O9 98.2(2) 7_445 6
Pb1 O7 O9 146.07(17) . 6
O9 O7 O9 59.9(2) . 6
Se3 O7 O1 171.5(4) . .
Cu3 O7 O1 45.59(19) 7_445 .
Pb1 O7 O1 51.70(18) . .
O9 O7 O1 135.3(2) . .
O9 O7 O1 135.3(2) 6 .
Se3 O7 O2 85.3(3) . 7_445
Cu3 O7 O2 40.62(17) 7_445 7_445
Pb1 O7 O2 137.9(3) . 7_445
O9 O7 O2 63.4(2) . 7_445
O9 O7 O2 63.4(2) 6 7_445
O1 O7 O2 86.2(3) . 7_445
Se3 O7 Cu6 68.51(18) . .
Cu3 O7 Cu6 63.62(15) 7_445 .
Pb1 O7 Cu6 145.47(15) . .
O9 O7 Cu6 34.57(12) . .
O9 O7 Cu6 68.12(17) 6 .
O1 O7 Cu6 104.0(2) . .
O2 O7 Cu6 32.75(9) 7_445 .
Se3 O7 Cu6 68.51(18) . 4_455
Cu3 O7 Cu6 63.62(15) 7_445 4_455
Pb1 O7 Cu6 145.47(15) . 4_455
O9 O7 Cu6 68.12(17) . 4_455
O9 O7 Cu6 34.57(12) 6 4_455
O1 O7 Cu6 104.0(2) . 4_455
O2 O7 Cu6 32.75(9) 7_445 4_455
Cu6 O7 Cu6 53.68(9) . 4_455
Se3 O7 Br4 111.11(15) . 1_565
Cu3 O7 Br4 56.94(8) 7_445 1_565
Pb1 O7 Br4 91.14(13) . 1_565
O9 O7 Br4 122.5(2) . 1_565
O9 O7 Br4 72.70(12) 6 1_565
O1 O7 Br4 65.34(11) . 1_565
O2 O7 Br4 67.56(11) 7_445 1_565
Cu6 O7 Br4 100.01(14) . 1_565
Cu6 O7 Br4 54.43(6) 4_455 1_565
Se3 O7 Br4 111.11(15) . .
Cu3 O7 Br4 56.94(8) 7_445 .
Pb1 O7 Br4 91.14(13) . .
O9 O7 Br4 72.70(12) . .
O9 O7 Br4 122.5(2) 6 .
O1 O7 Br4 65.34(11) . .
O2 O7 Br4 67.56(11) 7_445 .
Cu6 O7 Br4 54.43(6) . .
Cu6 O7 Br4 100.01(14) 4_455 .
Br4 O7 Br4 113.57(16) 1_565 .
Se3 O7 O4 123.1(3) . 7_445
Cu3 O7 O4 2.81(14) 7_445 7_445
Pb1 O7 O4 100.1(2) . 7_445
O9 O7 O4 95.8(2) . 7_445
O9 O7 O4 95.8(2) 6 7_445
O1 O7 O4 48.39(19) . 7_445
O2 O7 O4 37.82(17) 7_445 7_445
Cu6 O7 O4 61.20(13) . 7_445
Cu6 O7 O4 61.20(13) 4_455 7_445
Br4 O7 O4 57.15(8) 1_565 7_445
Br4 O7 O4 57.15(8) . 7_445
Se2 O8 Cu1 132.5(3) . 7_445
Se2 O8 Cu4 127.7(2) . 7_445
Cu1 O8 Cu4 93.91(17) 7_445 7_445
Se2 O8 O3 174.6(3) . 7_445
Cu1 O8 O3 49.61(15) 7_445 7_445
Cu4 O8 O3 47.93(15) 7_445 7_445
Se2 O8 O8 41.92(15) . 6_545
Cu1 O8 O8 165.55(14) 7_445 6_545
Cu4 O8 O8 98.02(11) 7_445 6_545
O3 O8 O8 137.60(14) 7_445 6_545
Se2 O8 O4 39.38(15) . .
Cu1 O8 O4 125.3(2) 7_445 .
Cu4 O8 O4 98.2(2) 7_445 .
O3 O8 O4 135.4(3) 7_445 .
O8 O8 O4 60.96(11) 6_545 .
Se2 O8 O1 88.42(18) . 7_445
Cu1 O8 O1 129.2(2) 7_445 7_445
Cu4 O8 O1 39.27(11) 7_445 7_445
O3 O8 O1 87.17(19) 7_445 7_445
O8 O8 O1 64.80(9) 6_545 7_445
O4 O8 O1 64.4(2) . 7_445
Se2 O8 Br2 87.77(17) . 7_445
Cu1 O8 Br2 45.27(10) 7_445 7_445
Cu4 O8 Br2 136.77(16) 7_445 7_445
O3 O8 Br2 94.80(16) 7_445 7_445
O8 O8 Br2 124.67(7) 6_545 7_445
O4 O8 Br2 97.20(18) . 7_445
O1 O8 Br2 153.5(2) 7_445 7_445
Se2 O8 Br5A 107.99(17) . 7_445
Cu1 O8 Br5A 111.61(19) 7_445 7_445
Cu4 O8 Br5A 62.61(12) 7_445 7_445
O3 O8 Br5A 73.33(16) 7_445 7_445
O8 O8 Br5A 67.52(7) 6_545 7_445
O4 O8 Br5A 121.30(17) . 7_445
O1 O8 Br5A 69.78(15) 7_445 7_445
Br2 O8 Br5A 135.99(15) 7_445 7_445
Se2 O8 Cu7 100.97(19) . 7_445
Cu1 O8 Cu7 92.67(17) 7_445 7_445
Cu4 O8 Cu7 98.81(17) 7_445 7_445
O3 O8 Cu7 83.45(19) 7_445 7_445
O8 O8 Cu7 77.51(8) 6_545 7_445
O4 O8 Cu7 136.82(17) . 7_445
O1 O8 Cu7 109.49(18) 7_445 7_445
Br2 O8 Cu7 96.97(13) 7_445 7_445
Br5A O8 Cu7 40.62(8) 7_445 7_445
Se2 O8 Cu4 72.01(13) . 4_445
Cu1 O8 Cu4 155.2(2) 7_445 4_445
Cu4 O8 Cu4 62.57(11) 7_445 4_445
O3 O8 Cu4 105.63(18) 7_445 4_445
O8 O8 Cu4 35.46(7) 6_545 4_445
O4 O8 Cu4 69.40(14) . 4_445
O1 O8 Cu4 33.36(8) 7_445 4_445
Br2 O8 Cu4 159.51(14) 7_445 4_445
Br5A O8 Cu4 52.25(7) 7_445 4_445
Cu7 O8 Cu4 84.02(11) 7_445 4_445
Se2 O8 Cu3 69.55(15) . .
Cu1 O8 Cu3 124.42(19) 7_445 .
Cu4 O8 Cu3 63.53(12) 7_445 .
O3 O8 Cu3 105.1(2) 7_445 .
O8 O8 Cu3 68.75(7) 6_545 .
O4 O8 Cu3 34.65(15) . .
O1 O8 Cu3 33.18(13) 7_445 .
Br2 O8 Cu3 122.30(14) 7_445 .
Br5A O8 Cu3 101.68(12) 7_445 .
Cu7 O8 Cu3 138.14(14) 7_445 .
Cu4 O8 Cu3 54.13(7) 4_445 .
Se3 O9 Cu6 124.6(2) . .
Se3 O9 Cu5 141.1(3) . .
Cu6 O9 Cu5 94.20(18) . .
Se3 O9 O2 171.6(3) . .
Cu6 O9 O2 46.99(15) . .
Cu5 O9 O2 47.25(15) . .
Se3 O9 O9 39.22(16) . 6
Cu6 O9 O9 97.44(12) . 6
Cu5 O9 O9 150.00(13) . 6
O2 O9 O9 135.76(14) . 6
Se3 O9 O7 39.13(15) . .
Cu6 O9 O7 96.8(2) . .
Cu5 O9 O7 145.4(2) . .
O2 O9 O7 134.9(3) . .
O9 O9 O7 60.06(12) 6 .
Se3 O9 O2 84.79(19) . 7_445
Cu6 O9 O2 39.86(12) . 7_445
Cu5 O9 O2 134.0(2) . 7_445
O2 O9 O2 86.84(17) . 7_445
O9 O9 O2 63.19(10) 6 7_445
O7 O9 O2 62.8(2) . 7_445
Se3 O9 Br3 99.24(19) . .
Cu6 O9 Br3 135.97(18) . .
Cu5 O9 Br3 41.82(9) . .
O2 O9 Br3 89.08(17) . .
O9 O9 Br3 121.93(7) 6 .
O7 O9 Br3 118.7(2) . .
O2 O9 Br3 174.87(17) 7_445 .
Se3 O9 Cu6 68.09(14) . 4_455
Cu6 O9 Cu6 63.09(11) . 4_455
Cu5 O9 Cu6 145.1(2) . 4_455
O2 O9 Cu6 104.84(18) . 4_455
O9 O9 Cu6 34.35(7) 6 4_455
O7 O9 Cu6 67.55(14) . 4_455
O2 O9 Cu6 32.60(9) 7_445 4_455
Br3 O9 Cu6 152.22(15) . 4_455
Se3 O9 O4 141.3(2) . .
Cu6 O9 O4 83.94(18) . .
Cu5 O9 O4 32.86(11) . .
O2 O9 O4 44.93(19) . .
O9 O9 O4 121.46(9) 6 .
O7 O9 O4 178.3(2) . .
O2 O9 O4 118.4(2) 7_445 .
Br3 O9 O4 59.96(13) . .
Cu6 O9 O4 114.16(15) 4_455 .
Se3 O9 Cu3 68.24(15) . 7_445
Cu6 O9 Cu3 62.52(12) . 7_445
Cu5 O9 Cu3 140.97(19) . 7_445
O2 O9 Cu3 104.1(2) . 7_445
O9 O9 Cu3 68.15(7) 6 7_445
O7 O9 Cu3 34.24(15) . 7_445
O2 O9 Cu3 32.48(14) 7_445 7_445
Br3 O9 Cu3 146.76(15) . 7_445
Cu6 O9 Cu3 53.32(7) 4_455 7_445
O4 O9 Cu3 146.42(18) . 7_445
Se3 O9 O9 140.78(16) . 6_545
Cu6 O9 O9 82.55(12) . 6_545
Cu5 O9 O9 30.00(13) . 6_545
O2 O9 O9 44.24(14) . 6_545
O9 O9 O9 180.0 6 6_545
O7 O9 O9 119.94(12) . 6_545
O2 O9 O9 116.81(10) 7_445 6_545
Br3 O9 O9 58.08(7) . 6_545
Cu6 O9 O9 145.65(7) 4_455 6_545
O4 O9 O9 58.54(9) . 6_545
Cu3 O9 O9 111.85(7) 7_445 6_545
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Pb1 O1 2.259(6) .
Pb1 O6 2.472(4) .
Pb1 O6 2.472(4) 6
Pb1 O7 2.493(6) .
Pb1 Br2 3.2597(12) 3
Pb1 Cu4 3.3702(10) .
Pb1 Cu4 3.3702(10) 6
Pb1 Cu3 3.3885(15) 7_445
Pb1 Br3 3.5617(10) 5_545
Pb1 Br3 3.5617(10) 5
Se1 O6 1.700(4) 6_545
Se1 O6 1.700(4) .
Se1 O5 1.729(7) .
Se1 O3 3.215(6) .
Se1 Cu4 3.2716(13) .
Se1 Cu4 3.2716(13) 6_545
Se1 Cu2 3.3269(18) 5_546
Se1 Cu2 3.3431(17) .
Se1 Br1 3.5467(15) 5_546
Se1 Br3 3.5564(17) 5_545
Se2 O4 1.687(7) .
Se2 O8 1.704(4) .
Se2 O8 1.704(4) 6_545
Se2 Cu3 3.3132(16) .
Se2 Cu1 3.3254(10) 7_435
Se2 Cu1 3.3254(10) 7_445
Se2 Cu4 3.3518(13) 4_445
Se2 Cu4 3.3518(13) 7_445
Se2 Br1 3.3852(17) 1_554
Se2 O1 3.389(6) 7_445
Se2 Cu5 3.4772(18) .
Se2 Br2 3.6376(11) 7_445
Se3 O9 1.691(4) .
Se3 O9 1.691(4) 6
Se3 O7 1.692(7) .
Se3 O2 3.226(6) 7_445
Se3 Cu6 3.2569(11) .
Se3 Cu6 3.2569(11) 4_455
Se3 Cu3 3.2917(16) 7_445
Se3 Cu5 3.5829(11) 1_565
Se3 Cu5 3.5830(11) .
Br1 Cu2 2.4441(16) .
Br1 Cu7 2.526(3) 4_446
Br1 Cu7 2.526(3) 7_446
Br1 Cu7 2.610(3) 6_545
Br1 Cu7 2.610(3) .
Br1 Cu1 2.9706(18) .
Br1 O3 3.129(6) .
Br1 O5 3.323(7) 5_546
Br1 Se2 3.3852(17) 1_556
Br1 Se1 3.5467(15) 5_546
Br1 O8 3.631(5) 1_556
Br1 O8 3.631(5) 6_546
Br2 Cu1 2.3619(16) .
Br2 Cu7 2.513(3) 7_446
Br2 Cu7 2.513(3) 4_446
Br2 Pb1 3.2597(12) 3_445
Br2 O8 3.281(4) 7_445
Br2 O8 3.281(4) 4_445
Br2 O6 3.515(4) 3_445
Br2 O6 3.515(4) 8_445
Br2 Se2 3.6376(11) 7_445
Br2 Se2 3.6376(11) 7_435
Br2 Br5B 3.792(15) 7_446
Br2 Br5A 3.945(2) 7_446
Br3 Cu5 2.3467(17) .
Br3 O9 3.450(5) .
Br3 O9 3.450(5) 6_545
Br3 O4 3.471(7) .
Br3 O6 3.540(5) 5_545
Br3 O6 3.540(5) 2
Br3 Se1 3.5564(17) 5_545
Br3 Pb1 3.5617(10) 5_545
Br3 Pb1 3.5617(10) 5
Br3 O7 4.206(4) 5
Br3 O7 4.206(4) 5_545
Br3 O2 4.254(6) .
Br4 Cu4 3.0183(13) .
Br4 Cu4 3.0183(13) 6_545
Br4 Cu3 3.1401(9) 7_435
Br4 Cu3 3.1401(9) 7_445
Br4 Cu6 3.3100(11) 4_445
Br4 Cu6 3.3100(11) .
Br4 O3 3.474(6) .
Br4 Cu1 3.5684(18) .
Br4 O1 3.582(3) .
Br4 O1 3.582(3) 1_545
Br4 O8 3.631(5) 7_445
Br4 O8 3.631(5) 4_445
Cu1 O8 1.928(4) 4_445
Cu1 O8 1.928(4) 7_445
Cu1 O3 1.947(6) .
Cu1 Cu4 2.8908(13) 6_545
Cu1 Cu4 2.8908(13) .
Cu1 Cu7 3.103(3) 7_446
Cu1 Cu7 3.103(3) 4_446
Cu1 Cu2 3.2844(18) .
Cu1 Se2 3.3254(10) 7_435
Cu1 Se2 3.3254(10) 7_445
Cu2 O3 1.878(6) .
Cu2 O5 1.947(6) 5_546
Cu2 O5 2.006(7) .
Cu2 Cu2 3.108(3) 5_546
Cu2 Br5A 3.1420(9) .
Cu2 Br5A 3.1420(9) 1_545
Cu2 Br5B 3.1495(16) .
Cu2 Br5B 3.1495(15) 1_545
Cu2 Cu4 3.1844(15) 6_545
Cu2 Cu4 3.1845(15) .
Cu3 O2 1.891(7) .
Cu3 O1 1.915(6) 7_445
Cu3 O7 2.001(6) 7_445
Cu3 O4 2.007(6) .
Cu3 Cu5 3.0625(18) .
Cu3 Br4 3.1401(9) 7_435
Cu3 Br4 3.1401(9) 7_445
Cu3 Cu6 3.1432(12) .
Cu3 Cu6 3.1432(12) 4_445
Cu3 Cu4 3.1663(14) 4_445
Cu3 Cu4 3.1663(14) 7_445
Cu3 Se3 3.2917(16) 7_445
Cu4 O1 1.905(4) .
Cu4 O3 1.906(4) .
Cu4 O6 1.973(4) .
Cu4 O8 2.027(4) 7_445
Cu4 Br5A 2.986(2) .
Cu4 Cu4 3.1014(16) 6
Cu4 Cu3 3.1662(14) 7_445
Cu4 Cu4 3.1672(16) 6_545
Cu5 O2 1.908(6) .
Cu5 O4 2.070(7) .
Cu5 O9 2.106(4) .
Cu5 O9 2.106(4) 6_545
Cu5 Cu6 2.9971(11) 4_445
Cu5 Cu6 2.9971(11) .
Cu5 Se3 3.5830(11) 1_545
Cu5 Br4 4.4617(14) 7_435
Cu6 O2 1.878(4) 7_445
Cu6 O2 1.878(4) .
Cu6 O9 1.983(5) 7_445
Cu6 O9 1.983(5) .
Cu6 Cu5 2.9971(11) 7_445
Cu6 Cu6 3.1343(9) 4_455
Cu6 Cu6 3.1343(9) 4_445
Cu6 Cu3 3.1432(12) 7_445
Cu6 Se3 3.2569(11) 7_445
Br5A Br5B 0.501(12) .
Br5A Cu7 2.331(4) .
Br5A Cu7 2.331(4) 6
Br5A Br5B 2.953(13) 5_556
Br5A Cu4 2.986(2) 6
Br5A Cu2 3.1420(9) 1_565
Br5A O8 3.315(5) 7_445
Br5A O8 3.315(5) 4_455
Br5A Br5A 3.421(5) 5_556
Br5A O3 3.546(3) 1_565
Br5B Cu7 2.495(14) .
Br5B Cu7 2.495(14) 6
Br5B Br5B 2.50(3) 5_556
Br5B Br5A 2.953(13) 5_556
Br5B Cu2 3.1495(15) 1_565
Br5B Cu4 3.338(12) 6
Br5B O5 3.559(7) 5_556
Br5B O5 3.559(7) 5_546
Br5B O5 3.618(8) 1_565
Cu7 Cu7 1.067(5) 6
Cu7 Br2 2.513(3) 7_446
Cu7 Br1 2.526(3) 7_446
Cu7 Cu1 3.103(3) 7_446
Cu7 Cu7 3.390(6) 7_446
Cu7 O8 3.397(6) 7_445
Cu7 Br1 3.674(3) 1_565
Cu7 O8 3.774(6) 4_455
O1 Cu4 1.905(4) 6
O1 Cu3 1.915(6) 7_445
O1 O6 2.641(6) .
O1 O6 2.641(6) 6
O1 O7 2.675(9) .
O1 O8 2.977(7) 7_445
O1 O8 2.977(7) 4_455
O1 O4 2.993(9) 7_445
O1 Se2 3.389(6) 7_445
O2 Cu6 1.878(4) 4_445
O2 O4 2.469(9) .
O2 O9 2.546(6) 6_545
O2 O9 2.546(6) .
O2 O7 2.890(9) 7_445
O2 O9 2.905(7) 4_445
O2 O9 2.905(7) 7_445
O2 Se3 3.226(6) 7_445
O2 O2 3.756(7) 7_445
O3 Cu4 1.906(4) 6_545
O3 O8 2.527(6) 4_445
O3 O8 2.527(6) 7_445
O3 O5 2.844(9) .
O3 O6 2.887(7) 6_545
O3 O6 2.887(7) .
O4 O8 2.611(7) .
O4 O8 2.611(7) 6_545
O4 O1 2.993(9) 7_445
O4 O9 3.495(7) .
O4 O9 3.495(7) 6_545
O4 Cu4 3.526(6) 4_445
O4 Cu4 3.526(6) 7_445
O5 Cu2 1.947(6) 5_546
O5 O5 2.444(13) 5_546
O5 O6 2.634(7) 6_545
O5 O6 2.634(7) .
O5 Br1 3.323(7) 5_546
O5 Cu4 3.482(6) 6_545
O5 Br5B 3.559(7) 5_556
O5 Br5B 3.559(7) 5_546
O6 O6 2.641(8) 6_545
O6 Cu4 3.501(4) 6_545
O6 Br2 3.515(4) 3
O6 Br3 3.540(5) 5_545
O6 O6 3.627(8) 6
O7 Cu3 2.001(6) 7_445
O7 O9 2.625(7) .
O7 O9 2.625(7) 6
O7 O2 2.890(9) 7_445
O7 Cu6 3.471(6) 4_455
O7 Br4 3.746(4) 1_565
O7 O4 4.003(9) 7_445
O8 Cu1 1.928(4) 7_445
O8 Cu4 2.027(4) 7_445
O8 O3 2.528(6) 7_445
O8 O8 2.536(8) 6_545
O8 O1 2.977(7) 7_445
O8 Br2 3.281(4) 7_445
O8 Br5A 3.315(5) 7_445
O8 Cu7 3.397(6) 7_445
O8 Cu4 3.460(4) 4_445
O9 O9 2.620(8) 6
O9 O2 2.905(7) 7_445
O9 Cu6 3.485(4) 4_455
O9 Cu3 3.520(5) 7_445
O9 O9 3.648(8) 6_545

_cod_database_fobs_code 2108346
